Author’s Accepted Manuscript The Forming Limit Curve for Multiphase Advanced High Strength Steels Based on Crystal Plasticity Finite Element Modeling Bassam Mohammed, Taejoon Park, Hyunki Kim, Farhang Pourboghrat, Rasoul Esmaeilpour www.elsevier.com/locate/msea

PII: DOI: Reference:

S0921-5093(18)30526-4 https://doi.org/10.1016/j.msea.2018.04.029 MSA36349

To appear in: Materials Science & Engineering A Received date: 2 January 2018 Revised date: 5 April 2018 Accepted date: 6 April 2018 Cite this article as: Bassam Mohammed, Taejoon Park, Hyunki Kim, Farhang Pourboghrat and Rasoul Esmaeilpour, The Forming Limit Curve for Multiphase Advanced High Strength Steels Based on Crystal Plasticity Finite Element M o d e l i n g , Materials Science & Engineering A, https://doi.org/10.1016/j.msea.2018.04.029 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting galley proof before it is published in its final citable form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.

The Forming Limit Curve for Multiphase Advanced High Strength Steels Based on Crystal Plasticity Finite Element Modeling Bassam Mohammeda, b, Taejoon Parkb, Hyunki Kimb, Farhang Pourboghratb,c *, and Rasoul Esmaeilpourb a

Department of Mechanical Engineering, Michigan State University, 428 S Shaw Ln, East Lansing, MI 48824, United States b

Department of Integrated Systems Engineering, The Ohio State University, 210 Baker Systems, 1971 Neil Avenue, Columbus, OH 43210, United States

c

Department of Mechanical and Aerospace Engineering, The Ohio State University, 201 W 19th Ave, Columbus, OH 43210, United States

April 05, 2018

* Corresponding author. Tel.: +1 (614) 292 3124; E-mail: [email protected]

1

Abstract A computationally efficient rate independent crystal plasticity finite element (CPFE) model was used to predict the forming limit curve (FLC) for a multiphase advanced high strength steel (AHSS). The CPFE model accounts for mechanical properties of the steel phases based on their individual plastic deformation and slip systems. The macroscopic behavior of the polycrystalline aggregate was predicted based on the volume-averaged response of the representative phases, and their volume fraction in the steel sheet. In addition to the random texture distribution assumption for each grain, the volume fractions of various phases were also assumed to be randomly distributed at each integration point. The microstructural inhomogeneity of the material, as well as a geometrical inhomogeneity in the form of a groove region in the specimen, based on the Marciniak-Kuczynski (MK) theory, were considered in the calculation of the FLC using the CPFE model (MK-CPFE). The validity of predicted FLC for quenched and partitioned QP980 steel was confirmed by comparing the results with experimental measurements. The FLC calculated by CPFE model showed that the presence of microstructural inhomogeneity allows for a more realistic prediction of the localized necking phenomenon. Subsequently, the FLC was used to compute the limit strains for the T-shape part stamping process. The limit strains and the punch force-stroke relationship for the T-shape part predicted by the multiphase CPFE model were in good agreement with experimental results.

Keywords: Finite element method, Crystal plasticity, Advanced high strength steel, Forming limit curve, Marciniak–Kuczynski analysis

2

1. Introduction Improved fuel economy, crashworthiness, and a higher stiffness for better drivability all require the application of higher strength materials with good combinations of strength, formability, fatigue resistance, and toughness. As a consequence of the increased demands on steels by automotive manufactures, new products referred to as “advanced high strength steels” (AHSS) have been developed and are now being utilized [1]. AHSS, such as dualphase (DP), complex phase (CP), transformation-induced plasticity (TRIP), and twinning induced plasticity (TWIP) are all multiphase steels which possess a composite microstructure comprised of ferrite, bainite, austenite, and martensite [2]. Consequently, AHSS derive their extraordinary properties from a complex, heterogeneous microstructure and the interactions between different phases.

With the advent of increased application of AHSS in automotive industries, new challenges in the sheet metal forming processes have surfaced, which further spawned new efforts in the fields of experimental, theoretical and numerical modeling. Part of these new initiatives included development and application of new constitutive models, failure criteria and friction models. Also, development of material data needed for the calibration of complex material models became imperative [3]. Understanding how the constituent’s phases in AHSS interact to achieve a desired strength, resistance to localized necking and fracture is particularly challenging. Moreover, volume fraction, grain morphology and micromechanical properties of the constituent phases play an important role during the material selection for automobile components. Therefore, formability assessments of AHSS require an understanding of the effects that material microstructure has on the forming limit strains, as well as on the operating deformation mechanisms.

Failure in sheet metal forming processes are often evaluated based on the onset of localized necking, which is characterized by the forming limit curve (FLC) in the principal strain space. FLC separates the region of uniform sheet deformation from the region of slightly greater deformation, where a local instability or a “neck” occurs [4]. The concept of FLC was pioneered by Keeler [5] for the tension-tension domain of the right hand side of the FLC, and extended by Goodwin [6] to the tension-compression domain. The FLC has been shown to be quite useful in representing the onset of sheet necking, and now is a standard tool for 3

characterizing the material forming behavior and a standard tool to study the formability of sheet metals.

Although the concept of FLC is simple to understand and apply, it has limited application. The actual response and failure of a material during the plastic deformation depends on a large number of coupled effects, making experimental determination of the material failure non trivial and time consuming [7]. In addition, scatter in the experimental data for a given sheet is often so large that researchers sometime question the accuracy and precision with which the FLC has been determined [8]. Experimental determination of the onset of diffuse necking becomes even more important when it comes to multi-phase AHSS sheets, since they are relatively new to stamping engineers.

In view of the continuous push to reduce development costs, considerable efforts must be made to develop microstructure sensitive constitutive models, as well as material instability criteria to assess AHSS sheet metal formability. Early theoretical models proposed by Swift [9] and Hill [10] describe diffuse and localized necking for a homogenous material, respectively. Marciniak and Kuczyński [11] proposed the MK model based on the premise that sheet metals are non-homogeneous from both geometrical and microstructural point of view. According to the MK model, an infinitely long sheet metal contains a local imperfection region (i.e. the grove), which is a band having an initial thickness less than that of the bulk sheet. These authors showed that the presence of such an imperfection could lead to unstable deformation in the grove region, and subsequently result in a localized necking and failure. The MK model has since been one of the most widely applied models for FLC prediction, and well established for predicting sheet metal necking among researchers [12].

In the last five decades, authors have been implementing various yield criteria and hardening rules in the MK model. A common observation is that FLC predictions are very sensitive to the choice of the constitutive model being used [13]. The MK model is frequently used with the quadratic Hill’48 [14] and the von Mises yield functions. However, both models overpredict the limit strains for biaxial paths. Sowerby and Duncan [15] used Hill’48 yield criterion and the Swift type isotropic hardening law [9] to calculate the FLC. They showed that the right-hand side of the FLC increases with an increase in the stain hardening exponent 4

(n-value), and its shape is slightly affected by the normal anisotropic parameter (r-value).

Several non-quadratic yield functions have been developed and subsequently implemented for computational modeling and prediction of limit strains. Graf and Hosford [16,17] predicted the right-hand side of the FLC with the MK analysis using the non-quadratic Hosford yield criterion [18]. The computed FLC was found to increase by increasing the nvalue, and was unaffected by the r-value. The predicted FLC using Hosford yield criterion, although still higher, was in better agreement with the experimental FLC, compared with results obtained with Hill’48 yield criterion. Barlat et al. [19] calculated FLCs for one aluminum and two steel sheets using the Yld94 yield function. Their predictions were in reasonable agreement with experimentally measured FLCs. Cao et al. [20] predicted FLC based on the MK analysis using the K-B yield function developed by Karafillis and Boyce [21], and analyzed the effect of changing the strain-paths on the FLC. An algorithm proposed by Ávila and Vieira [22] was used to predict the right-hand side of the FLC using the methodology proposed by Marciniak and Kuczynski using five different yield criteria. They confirmed that the type of yield criterion used in the analysis strongly influences the FLC. More recently, additional contributions have been made in predicting FLC curves based on the MK analysis using more complex phenomenological models [23–31].

In the MK model, instability is viewed as a process in which the strain state in a small region of the material (i.e., grove) evolves to one of plane strain as deformation proceeds uniformly in the rest of the material (i.e., bulk). In general, this characteristic agrees well with the experimentally observed failures in sheet metals. However, the analytical MK model is based on simplified assumptions, such as the defect is infinite in length and boundary effects are not accounted for. The analytical MK analysis, therefore, implicitly imposes nonphysical boundary conditions by way of assuming uniform minor strains throughout the sample sheet. These two simplifications allow for the derivation of closed form one-dimensional solutions when allowing variations in the field quantities to occur in one direction only [32]. Finite element modeling allows relaxation of these two restricting assumptions by solving for nonuniform internal stresses and strains under prescribed displacement boundary conditions. Therefore, researches have been using phenomenological models and finite element method (FEM) to computationally calculate limit strains within the framework of the MK model 5

(MK-FEM). Narasimhan and Wagoner [33] used the FEM approach to predict the FLC of a sheet specimen with finite defect in the middle of the sheet far from the applied boundary condition. They studied numerous material aspects and their effects on the predicted FLC, as well as validated their results with analytical MK model. However, with an imperfection factor less than 0.98, the strain paths in the groove region showed an earlier deviation from the applied strain path of the bulk and eventually tended to plane strain. This is in contrast with the MK model where the strain path of the groove stays proportional at the beginning and deviation occurs much later. In the MK-FEM, in addition to the imperfection factor, the aspect ratios of the initial groove and the bulk have a significant influence on the rate of strain localization and thus on the predicted FLCs. These effects were not taken into account by some researchers in their MK-FEM, and the imperfection factor was the only parameter used for predicting FLC using different phenomenological models [34–36]. Recently, Srivastava et al. [37] predicted the FLC of two DP steels based on the standard ratedependent, isotropic plasticity model (von Mises), and MK-FEM. The flow behavior of DP steel used for the FLC prediction was calculated with finite element simulation coupled with a microstructure-based crystal plasticity model. In their study, the imperfection factor and the aspect ratio of the groove were only determined from the measurements of the surface roughness of the sheets using a three-dimensional (3D) digital image correlation (DIC) technique. It was found that the prediction of FLC via their method was in good agreement with experimental results only within a limited strain range.

Phenomenological models can describe the effects of initial anisotropy; however, they still have some difficulty accounting for the evolution of the yield surface. In addition, they can be very arduous to calibrate, requiring many experiments and are only valid for monotonic loading. For complex metal forming, the assumption of monotonic loading for predicting limit strains is not adequate [38]. It is well known and widely recognized that the crystallographic texture evolution strongly affects the FLC and the macroscopic anisotropy of polycrystalline sheet metals. Research has shown that the localization of the plastic flow is influenced by deformation-induced textures and anisotropy [39]. Thus, more realistic constitutive models, often involving crystal plasticity, are preferable. These microstructurebased models provide a framework to better understand the relationship between flow localization and the material’s microstructure, and their impacts on forming limits. Issues 6

such as material anisotropy, shape of the yield-surface and crystal orientation can be directly addressed by using a microstructure-based constitutive model.

Zhou and Neale [40] predicted FLCs for annealed aluminum sheet using an analytical polycrystalline model based on Taylor homogenization scheme and the analytical MK model [41]. Many recent studies have employed crystal plasticity models for predicting FLCs for sheet metals based on a single-phase assumption. It is well documented that factors such as the initial imperfection, texture, hardening rate, temperature, and the choice of the constitutive model affect the prediction of FLC [7, 39, 43–57].

The analytical prediction of FLC based on crystal plasticity and MK analysis with more than one phase are scarce in the literature. In a recent study by Schwindt et al. [4,56] the authors investigated formability prediction of DP780 steel with only body centered cubic (BCC) structure (ferrite and martensite). In their study, due to the lack of experimental flow curves for ferrite and martensite, four simulated uniaxial flow curves for these phases were calibrated by matching the experimental flow curve for DP780. Also, because of the high computational cost related to using Visco-Plastic Self-Consistent (VPSC) model in their study, only limited number of orientations were assumed. However, they noted that even when they used thousands of orientations for multiple phases in the steel, the FLCs predicted by MKCPFE model showed, to some extent, sensitivity to the phase distribution.

The typical FLCs for cold rolled QP980, DP780 and DP980 steel sheets have been reported by Wang and Speer [57]. The authors showed that the formability of QP980 is superior to that of DP980 steel, and reaches similar levels as that of DP780. Recently, the formability of three DP980 steels and one QP980 steel was evaluated by Zhang et al. [58] using hemispherical punch tests and DIC technique. Inconsistent and scattered results were observed when they compared the formability of the four AHSS sheets based on the commonly used FLC method. According to their observations of the strain distribution in the hemispherical punch tests and metallurgical analysis of the QP980 steel, the inconsistency and scatter in the formability was attributed to the microstructural features of the sheet metal. They observed that strain valleys occur in the regions with higher martensite volume fraction, and conversely strain peaks occur in regions with a lower volume fraction of martensite. The authors proposed an 7

analytical method based on mathematical expectation and variance to evaluate the formability of sheet metals and correlate them to the global strain distribution observed in DIC. Also, they concluded that the application of traditional formability evaluation methods might not be suitable for the newly developed steel sheets with complex multiphase microstructure. Also, Mohammed et al. [59] numerically studied the formability of QP980 steel using multiphase crystal plasticity simulation of hemispherical punch tests. The authors concluded that the inhomogeneous deformation and formation of strain bands in the steel sheet are related to the inhomogeneous phase distributions, and that it had significant impact on the FLC prediction, and on the scattering observed in the experimentally predicted FLCs.

The most reliable method to numerically predict the FLC for sheet metals is to simulate the hemispherical punch test with similar boundary conditions and specimen sizes used in the experiments. However, given the complex geometry of the hemispherical punch test and specimen shapes, and highly intensive computational time, especially with crystal plasticity finite element method (CPFEM), it was opted in this study to use the simpler rectangular geometry of the specimen used in the MK analysis for the FLC prediction. It was found that the analytical prediction of FLC using MK model in conjunction with crystal plasticity and Taylor homogenization scheme does not accurately predict the forming limits. The main shortcoming of this analytical approach was identified to be its assumption that all crystal orientations exist and evolve at only one material point, and therefore crystal orientation and phases distribution of the specimen cannot be accounted for. In contrast, by using FEM to predict forming limits, multiple integration points with different orientation distributions can be assumed to more accurately represent microstructural properties of the sheet metal. Also, by using FEM to predict FLC, it is possible to impose the more natural boundary conditions, such as displacement or velocity, rather than strains, which are imposed in the analytical model.

Present research focuses on the prediction of the FLC for multiphase AHSS sheet based on the CPFE modeling and the MK theory (MK-CPFE). More specifically, the influence of geometrical and material inhomogeneity on the FLC for AHSS sheet is studied, and some viewpoints about the FLC predictions are expressed based on these two characteristics. The inhomogeneity of various phases within the steel sheet is considered through the crystal 8

plasticity constitutive relationships based on crystallographic slip systems, which not only accounts for the initial elastic–plastic anisotropy, but also for its gradual evolution during the forming process due to the texture evolution. The verification of the accuracy of the adopted method in this study was investigated based on the comparison of predicted and experimental results, in terms of hemispherical punch tests and the stamping of the T-shape component.

2. Crystal Plasticity Constitutive Models The rate-independent crystal plasticity model used in this study was first presented by Zamiri and Pourboghrat [60] for single materials and was recently modified by Mohammed et al. [59] for multiphase metals. A brief summary of the important components of the formulations are presented in this section. The formulations were implemented into the commercial finite element program Abaqus/Explicit via a user material subroutine VUMAT.

2.1. Crystal plasticity yield function In the crystal plasticity model [60], the yield function is defined as:

f (σ, q)

where is the slip system, N

N | σ : P | ln exp 1 1 m y 1

(1)

is the number of slip systems, y is the critical resolved

shear stress (CRSS), ρ is a parameter to determine the closeness to the condition,

| σ : P | y , and m is a parameter for a flexible yield function shape. Also, Pα is a matrix of the Schmid tensor and I describes the orientation of a slip system, defined as:

1 P [m n (m n )T ] 2

(2)

where n is a unit vector representing the normal to the slip plane, and m is a unit vector denoting the slip direction. The plastic deformation gradient can be expressed as: N

DP P 1

9

(3)

where are the shear slip rates. The spin tensor, which represents the material rotation due to slip, can be expressed as: N

P ω

(4)

1

where ω matrix is the anti-symmetric part of P , defined as:

1 ω [m n (m n )T ] 2

(5)

The slip rate on any slip system can be expressed by: σ : P exp 1 y m y σ:P N m exp 1 m y 1

sgn(σ : P )

(6)

where represents the index of summation for slip systems, m and are material parameters that control the shape of the single-crystal yield surface, which have been shown to have a direct relationship with the stacking fault energy of the material. 2.2. Hardening model In order to define the resistance against shear stress, an extended Voce type strain hardening type [61] was used:

0 1

y () 0 1 1 1 exp

(7)

where is the total accumulated shear strain over the entire deformation, and y is the critical resolved shear stress on the slip system as a function of . The initial yielding is 10

characterized by 0 , and 0 is the hardening rate, while the asymptotic hardening is characterized by 1

and 1 . The extended Voce model represents the exponential

hardening which consists of the initial critical resolved shear stress, 0 , and the work hardening rate, 0 . The excess stress 1 can be obtained before the critical resolved shear stress reaches saturation where the sum of 0 and 1 is the saturation stress at which the work hardening rate approaches zero. The 1 represents a constant work hardening rate for the linear hardening part of extended Voce-law. The total accumulated shear strain on all slip systems , can be defined as:

N 1

dt

(8)

2.3. Homogenization method In the present study, the Taylor type homogenization was used for the calculation of the homogenized stress in case of multiple grains were considered for each integration point in the finite element simulations. According to the Taylor model, which is an upper bound model, each grain of the polycrystal aggregate undergoes the same deformation and deformation rate. Therefore, the deformation gradient in Eq. (3) in all grains are the same and equal to the overall deformation gradient.

By assuming that grains have the same volume V c for simplicity, the homogenized stress,

σ , can be calculated from the crystal stress σ c : σ

Vc V

σ

c

c

1 M

σ

c

(9)

c

where V is the total volume of grains, and M is the number of grains [62]. For multiphase materials, Eq. (9) can be rewritten in the form:

1 σ fi i 1 Mi

11

σ c

i c

(10)

where fi is the volume fraction of each phase. Eq. (10) is then used in the explicit algorithm to calculate the macroscopic stress tensor from the crystal stress tensors for all phases. 2.4. Crystal orientation For the material texture representation, the three Euler angles 1 , and 2 that are defined based on Bunge convention to define the orientation of any crystal with respect to the material coordinate system is used [63]. Based on the Bunge system, the orientation of a crystal can be defined by the three Euler angles to create a rotation tensor Q as, sin 1 sin 2 cos 1 sin 2 cos sin 2 sin cos 1 cos 2 sin 1 sin 2 cos Q(1 , , 2 ) cos 1 cos 2 sin 1 sin 2 cos sin 1 sin 2 cos 1 cos 2 cos cos 2 sin sin 1 sin cos 1 sin cos

(11)

3. Material Characterization In this study, to verify the accuracy of the proposed methodology for predicting FLC based on CPFE, numerically generated results were validated against various experiments conducted with the QP980 sheets. The strain hardening characteristics of the steel were determined using uniaxial tension tests performed along the rolling direction. Experimental results from a hemispherical punch test were also compared with numerically predicted results to verify the accuracy of the proposed methods. The tensile and hemispherical punch test procedures have been discussed in details in Mohammed et al. [59], for the sake of completeness, these experimental procedures and relevant results for the QP980 are summarized briefly in the present work. Also, this section summarizes the properties of the QP980 used in this work as well as the calibrated hardening parameters with the uniaxial flow curve for parent QP980 and its constituent’s phases.

3.1. Mechanical and microstructure behavior The uniaxial tensile behavior of the QP980 steel sheet was measured using a universal tensile testing machine. ASTM E8 [64] standard tensile specimens were used to measure stressstrain curves in the rolling direction (RD), diagonal direction (DD), and transverse direction (TD) (or 0o,45o, and 90o to RD, respectively) at the nominal strain rate of 0.002 s-1. For strain 12

measurements, a 3D system DIC technique ARAMIS 5M was used to monitor the deformation of the test specimens. The uniaxial tensile stress–strain curves for the QP980 at room temperature with different alignment to the RD are shown in Fig. 1. This figure also shows the QP980 sheet’s microstructure inhomogeneity as bands appearing on its surface detected by DIC along diagonal and transverse directions at 4% strain.

Fig. 1: Uniaxial tensile stress–strain curves for the QP980 sheet steel with loading axis aligned parallel, diagonal (DD) and normal (TD) to the rolling direction (RD).

The optical micrographs taken from the middle of the sheet for cross sections perpendicular to the TD and perpendicular to the RD are shown in Fig. 2(a) and (b), respectively. It can be seen that the spatial distribution of martensite (dark regions) is not uniform. Such martensite morphology and inhomogeneous distribution had a significant influence on the accumulation of strains in soft phases such as ferrite (light regions) and subsequently on FLC prediction.

13

(a)

(b)

Fig. 2: Micrographs taken from cross sections of the QP980 sheet showing the size of the martensite band (dark regions) in the microstructure. (a) perpendicular to the transverse direction (TD) and (b) perpendicular to the rolling direction (RD).

3.2. Hemispherical punch test The Hemispherical punch tests were conducted at room temperature to study the formability of QP980. Different blanks with varying width ranging from 20 mm up to 180 mm, and a 1.0 mm gauge thickness were stretched by the hydraulic displacement of the punch at a constant tool velocity of 1 mm/s [65]. A 3D DIC system was employed to measure strain histories on the blank’s surface. The formability of the QP980 was then evaluated based on FLC which was constructed by using the linear best fitting (LBF) method [59].

3.3. T-Shape component stamping The T-shape stamping was used in the present research to validate proposed methods for predicting the FLC based on multiphase CPFE model. This test was speciﬁcally designed to closely replicate actual forming conditions experienced by the sheet metal during the continuous stamping production. The T-shape stamping of 1.0 mm thickness QP980 steel sheets were carried out using Interlaken Servo-Press 150 system. Fig. 3(a) shows the tooling and the experimental setup, and Fig. 3(b) shows two different blanks used in the experiments: with and without holes. The formability of QP980 steel was investigated under a constant binder load of 20.0 Ton, and a punch speed of 0.1 mm/s. The T-shape stamping process took place in two steps: first a constant binder load was applied on the blank, and then the T-shape was formed under the actions of die and punch.

14

(a)

(b) Fig. 3: (a) The sheet metal stamping press tool components setup; (b) Dimensional characteristics of the specimens used in the T-shape experiments.

3.4. Calibration of the material parameters 3.4.1. Phenomenological model The von Mises yield function with isotropic hardening was used in this study to represent the plastic deformation of QP980 steel sheet. The properties of the von Mises yield function were determined using the uniaxial tensile data along the RD. The isotropic elastic constants used for the QP980 steel sheet were determined as C11 =269.23 GPa, C12 =115.38 GPa, and C44 =76.92 GPa. Uniaxial tension data along the RD was considered as the reference state for characterization of the Swift type isotropic hardening law [9]:

15

K ( 0 )n

(12)

where and are the effective stress and equivalent plastic strain, respectively, while K,

0 and n are the hardening coefficients. The hardening coefficients were determined using the least square method based on the experimental true stress-plastic strain curve along the RD. The following material parameters have been obtained: K = 1413.64 MPa, 0 = 2.1192×10-3 and n = 0.099. 3.4.2. Crystal plasticity model The material properties used to generate the simulated stress–strain curves of constituent phases are obtained by curve fitting uniaxial stress–strain simulations by crystal plasticity to experimental results. The experimental data from the in-situ high energy X-ray diffraction (HEXRD) test were used for the calibration of the parameters of the hardening model. These hardening parameters were fitted to each phase using the calibration method detailed by Mohammed et al. [59] and are listed in Table 1. [66,67]

Table 1. Material parameters for the CPFE model composed of four phases in QP980 steel (unit: MPa)

Martensite

0 348 487

1 130 55

0 1100 1994

1 117 185

Austenite

600

2

1600

550

New Martensite

496

39

2200

1788

Phase Ferrite

Fig. 4 shows the comparison between the experimental stress-strain curves for individual phases with the curves predicted by the CPFE model with 60 grain orientations assumed per gauss point for individual phases. Fig. 4 also shows the comparison between predicted and experimental macroscopic stress-strain curve for QP980 steel.

16

Fig. 4: Comparison of the experimental strain–stress curve with the CPFE model with 60 grain orientations assumed for each constituent phase and the QP980.

The effect of changing the number of grain orientations assumed per integration point on computed stress-strain curves for the case of uniaxial tensile test is shown in Fig. 5. It was also shown by others that increasing or reducing the number of grain orientations per integration point will have little impact on the macroscopic stress-strain curve [62,68].

17

Fig. 5: Comparison of the experimental strain–stress curve with the CPFE model in terms of the number of grain orientations assumed per integration point.

4. FLC Determination Procedures Based on Finite Element Simulation In this section, a multi-scale computational framework based on MK theory [11] and CPFE model (i.e., MK-CPFE) is developed to predict FLC for multiphase steel sheets. Similar to MK theory, the right-hand side of FLC is determined with CPFE using a rectangular specimen with a groove in the mid-section. To determine the appropriate geometry of the rectangular specimen, however, a number of finite element simulations were first performed with von Mises yield function (i.e., MK-FEM) to study the sensitivity of predicted FLC to geometrical parameters discussed in Section 4.1. Finally, the left-hand side of FLC was determined with only one point obtained from the CPFE simulation of the uniaxial deformation of a narrow specimen with a hemispherical punch test, and the LBF method [59] . 4.1. The finite element procedure and the failure criteria In the MK model, an imperfection, or a groove, is assumed to exist initially in the sheet metal as illustrated in Fig. 6(a). In real materials, however, numerous imperfections are present at arbitrary angles, and therefore, imperfections aligned at different angles should be considered for obtaining more accurate results. However, due to the inhomogeneous phase distributions in the QP980 sheet (Fig. 1), the localized strain and fracture were mostly observed to take place along the RD in the experiments [59]. Therefore, for the sake of simplicity and computational cost reduction, only an imperfection parallel to the RD, which corresponds to the x1 axis in Fig. 6(a), was considered for the calculation of the right-side of FLC based on the MK-FEM model.

In this study, a sheet specimen with the bulk thickness of t0b , width (dimension along x1) of 2W, and a total length (dimension along x2) of 2L was considered, as shown in Fig. 6(a). The Cartesian tensor notation was used, and the origin of the coordinate system was taken to be at the center of the specimen (i.e. sheet specimen was oriented so that the x1, x2, and x3-axes were parallel to the RD, TD, and normal direction (ND) of the sheet material, respectively). In order to reduce the computational cost, symmetric boundary conditions along x1 and x2 18

axes were assumed for regions 0 x1 W and 0 x2 L , so that only one quarter of the sheet specimen was needed for computational modeling, as shown in Fig. 6(a).

The commercial software MATLAB was used to generate different dimensions for groove and bulk regions. The dimensional values were then used in the mesh generation, creation of a FE model, and subsequent simulations with the commercial software ABAQUS [69]. Solid elements were used for FE simulations as illustrated in Fig. 6(a), with fine symmetric mesh (0.05 mm × 0.05 mm elements) in the groove region. A gradual increase in the mesh size in the bulk region, along x2 direction from 0.1 mm to 0.4 mm, was assumed in order to increase computational efficiency. To have a smooth transition of strains between the bulk and groove, a transition region with one element (0.1 mm thickness) was adopted, as shown in Fig. 6(b). The generated strains in the transition region were neglected in the analysis since they did not represent either the bulk or the groove region.

In all the MK-FEM simulations, the nominal thickness of the specimen in the bulk region was assumed to be t0b =1.0 mm, which corresponds to the measured average thickness of the QP980 sheets used in all the experiments. Also, the specimen width (W) was fixed to 3 mm length. The other two in-plane dimensions, Lg and Lb were iteratively adjusted until the best values for the bulk and groove aspect ratios (ARb and ARg) were found, such that the MKFEM predicted FLC matched the FLC calculated by analytical MK model. The selected parameters were chosen such that a direct comparison with the analytical MK model could be made. Therefore, the following three-groove aspect ratios (ARg) were considered, 4, 6, and 7.5, in the MK-FEM simulations. In addition, three aspect ratios for the bulk region were assumed for calibration. To determine the thickness of the groove region, it was gradually reduced until strain localization occurred inside of the imperfection area. The initial thickness of the groove region is given by: t0g f 0 t0b

19

(13)

where f 0 is the inhomogeneity factor, t0g and t0b are initial thicknesses of the groove and bulk, respectively. The sheet specimen was deformed under in-plane biaxial straining by prescribing the displacements d1 and d2. Therefore, the state of biaxial stretching was imposed as following:

1 2

0 1

(14)

where is the strain ratio corresponding to the deformation path, 1 and 2 are strains caused by imposing displacements d1 and d2 on planes A1 and A2, respectively, as shown in Fig. 6(a) and (b). It is important to mention that by imposing uniform displacements d1 and d2 in the FEA, only proportional engineering strains will be developed, and not the proportional true strains needed to construct FLC. To get around this problem, non-uniform displacements d1 and d2 had to be generated analytically first, and then imposed in the MK-FEM simulations to generate proportional true strains throughout the deformation. Fig. 6(c) visually shows the difference in proportionality between engineering and true quantities generated by assuming that 0.5 in engineering quantities (blue line). From the non-proportional engineering strain history, true strain history was converted and illustrated in red line, which can clearly show that the proportionality in true strains were maintained.

20

21

(c) Fig. 6: (a) Schematic of the undeformed finite element mesh, representing full and one quarter of sheet blank. The sheet blank is subjected to biaxial straining by applying displacements, d1 and d2 and symmetric boundary conditions; (b) Schematic of a sheet characteristics and dimensions; (c) A comparison between the engineering and true strains histories on the prediction of FLC for 0.5 .

During initial stages of the biaxial stretching of the sheet simulations, the sheet deformed uniformly in both the bulk and groove regions. However, as plastic deformations increased, a strain gradient developed and strains inside the groove region grew much faster than in the bulk region, resulting in a localized neck. To predict the limit strains from the groove region corresponding to the formation of a neck, the failure criterion was used. The FLC was then constructed by repeating the simulations for several different strain paths (i.e., 0 1 ), and plotting the principal strains in the bulk region once the assumed failure criterion was reached. In this study, the failure criterion was based on the onset of necking, identified as:

22g b 22

22

10

(15)

where,

g 22

1 Ng

22b

1 Nb

Ng

n 1

Nb

g n 22

(16)

n 1

b n 22

(17)

The sum of 22 in equations (16) and (17) is taken over all elements within groove and bulk regions, respectively. Ng and Nb are the total number of elements in groove and bulk regions, respectively.

The value of

22b

at the onset of necking in Eq. (17) will be referred to as the ‘major strain’

and the corresponding value of

11b

b (analogous to 22

in Eq. (17)) will be referred to as

the ‘minor strain’ for construction of FLCs. To predict FLCs of the steel sheet based on von-Mises model, FE simulations of in-plane biaxial straining of the steel sheet specimen characterized by varying aspect ratios of the groove and the bulk were carried out. These simulations used the calibrated hardening parameters based on the Swift type model shown in Eq. (12).

4.2. Crystal plasticity finite element procedure for phases implementation AHSSs have a considerably complicated microstructure, and their mechanical behavior cannot be explained by simple models, such as those proposed for metal-matrix composites [70]. Thus, applying a more complex constitutive model, such as crystal plasticity that accounts for microstructural properties, is required. However, when simulating complex deformation of steels, some simplifying assumptions must be made about texture to keep the CPFEM computational costs reasonably low, without sacrificing accuracy.

The experimental observations of the QP980 steel sheet revealed that this material is comprised of 44±2% by volume of martensite, ~8–10% by volume of retained austenite, and the rest ferrite. Using this information, the overall microstructure of QP980 steel sheet was 23

modeled with CPFE based on 45% ferrite, 45% pre-existing martensite, 5% retained austenite, and 5% transformed martensite. In the absence of an austenite to martensite phase transformation model in CPFE, it was assumed that a 5% new (transformed) martensite exists in the undeformed sheet from the beginning of deformation. However, in the real material, the volume faction of the new martensite evolves with increasing plastic strain. The assumption of having 5% new martensite available from the beginning of the deformation will not affect the material behavior in a significant way, since the newly transformed martensite will have low volume fraction compared to many TRIP steels.

Based on the EBSD data presented for the QP980 steel sheet in [59], it was concluded that assuming a random crystallographic orientation for aggregate grains is reasonable. Also, the slip systems used in the CPFEM for the deformation of BCC crystals (ferrite, old martensite, and new martensite) were (12 {110} and 12 {112} slip systems), while the following 12 slip systems ({111} slip systems) were considered for the FCC crystal (retained austenite). Finally, in this study, it was attempted to model the multiphase QP980 steel in such a way to represent its real microstructure and inhomogeneities. Therefore, a random phase distribution was assumed at each integration point, but the total distribution for each phase in the sheet was maintained at 45% ferrite, 45% old martensite, 5% austenite, and 5% new martensite. In other words, not every FE integration point had the same volume fraction of each phase. This scheme was adopted for prediction of FLC with the CPFE model, and for the simulation of the T-shape stamping. 5. Results and Discussion 5.1. Aspects ratios calibration with analytical MK model Forming limits of the steel sheet under biaxial stretching were calculated using the framework described in Section 4.1. The calculated forming limits based on von Mises and MK-FEM were compared with the calculated data based on the analytical MK model. The predicted FLCs based on changing the aspect ratio of the groove, ARg, and imperfection factor, f 0 , for a fixed bulk aspect ratio of ARb 3 5 , are shown in Fig. 7(a)-(c). 24

(a)

(b)

25

(c) Fig. 7: Comparison between the predicted FLCs based on analytical MK model and MKFEM for different groove aspect ratios with fixed bulk aspect ratio ( ARb =3/5); (a) f 0 =0.992; (b) f 0 =0.994; (c) f 0 =0.996.

From the comparison of the relative positions of the different curves in Fig. 7, it is apparent that the size of the groove as characterized by the ARg , for a given f 0 , influences the level of the FLC. The conclusion is that a defect (groove) can cause a strain localization that is controlled by both f 0 and its aspect ratio ( ARg ) . Compared with the analytical MK model, the MK-FEM model overestimates the magnitude of FLC0 (plane strain) as the assumed groove aspect ratio becomes larger than 4. For example, as shown in Fig. 7(c), for f 0 =0.996 and ARg =7.5, the FLC0 computed by FEM is on average 13% larger than those computed by the analytical MK model. This is an expected result as the assumed analytical MK defect is more severe for a given sheet thickness than the defect assumed in the MK-FEM model, and hence the plastic deformation localizes faster. Therefore, the ARg for the MK-FEM model must be adjusted to match the specified FLC0 for a given material. 26

The FLC calculated by the MK-FEM model with the ARb 1.0 , predicts forming strains that are slightly larger than those predicted by the analytical MK model for ρ less than 0.5, as shown in Fig. 8. Less sensitivity was noticed when the values of ARb reduced to 3/5 and 3/7.

Fig. 8: Bulk’s aspect ratio (ARb) effects on the of predicted MK-FEM forming limit curve for fixed groove aspect ratio (ARg=4) and imperfection factor (f0=0.992).

The effect of the aspect ratios on FLC predictions can be summarized as follows; increasing the value of ARg increases the values of the limit strains, whereas the values of the limit strains decrease when the values of ARb increases. However, the values of the limit strains are less sensitive to the changes in ARb compared with the changes in ARg values. The shape of analytical MK and MK-FEM FLCs are nearly identical for strain paths in the range of 0 ≤ ≤ 0.5, and FLC0, except for strain paths in the range of

0.6 ≤ ≤ 1, as

shown in Fig. 7. The comparison between various strain paths in groove and bulk regions is also shown in Fig. 9 for five different cases. The respective strain paths for the groove and 27

bulk calculated from the analytical MK model generally match the strains paths predicted by MK-FEM. However, small deviation can be observed in the cases of > 0.6.

Fig. 9: Comparison of the predicted MK-FEM and analytical MK model strain paths for an imperfection factor f0=0.992. As mentioned, the deformation behavior in the groove and the adjacent bulk with MK-FEM and analytical MK model is different because of the nonuniformity introduced by the presence of finite dimensions of groove and bulk with MK-FEM. Therefore, all limit strains from MK-FEM are not expected to have similar values to those predicted by analytical MK model due to the uniqueness of each model. Hence, the calibration method with analytical MK model was proposed here to find the best parameters that give approximate limit strains to that calculated by MK-FEM, and subsequently avoid choosing arbitrary dimensions that may affect the FLC prediction by adopting different constitutive models.

As expected, the FLCs calculated by MK models (analytical MK and MK-FEM), using von Mises and Swift type model for QP980 showed low plane strain (FLC0) value, and high balanced biaxial strain limits, which is inconsistent with what was observed from 28

experimental results of QP980 steel [57–59]. It should be mentioned that FLC predicted by MK models (analytical MK and MK-FEM) is the combined result of the assumed failure model and the consitututive model that describes material properties and behaviour under plastic deformation. In the next section, it will be shown that by adopting a more sophisticated material model (crystal plasticity), but the same failure model described in Section 4.1. , more accurate results that better fit experimental measurments can be obtained.

5.2. FLC prediction based on MK-CPFE It is well known that a slight change in the shape of the yield surface for a sheet metal can have a rather large effect on predicted FLC [71]. In the MK-CPFE forming limit curve analysis carried out here, beside the mechanical properties of various phases, the shape of the ‘yield surface’ for the sheet metal is specified by the assumed initial texture, as well as its evolution.

The MK analysis predicts the FLC based on the growth of an initial imperfection factor f 0 . However, the strength of the imperfection cannot be directly measured by physical experiments. Thus, it is possible to predict the experimentally observed FLC0 by a suitable choice of the f 0 . In other words, since f 0 has no physical meaning, it is simply a fitting parameter that allows a model to be calibrated by matching the experimentally measured FLC0. Here, the lowest initial imperfection factor ( f 0 =0.992) and the initial aspects ratios of ARg = 4 and ARb = 3/5 were chosen for the FLC prediction based on MK-CPFE. These

values showed the best fit for the lowest strain limit in plane strain condition (FLC0) of the QP980 steel.

The initial texture (represented by 912,000 grains) with 20 grains per integration point was employed in the FLC simulations, as shown in Fig. 10(a). The orientations and volume fractions of phases were distributed randomly in all integration points. Fig. 10(a) shows two different strategies to model FLC based on random distribution of phases. FLC1 was predicted by using the same randomly generated volume fraction and orientation distributions in all integration points for all strain paths ( 0 1 ). On the other hand, FLC2 was predicted by using different randomly generated volume fraction and orientation distributions 29

in all integration points for all strain paths ( 0 1 ). In the second method, the material subroutine (multiphase CPFE-VUMAT) randomly generated a new volume fraction of phases and orientation distributions for each simulation run. In all the simulations, however, the volume fraction of phases were kept at 45% ferrite, 45% old martensite, 5% austenite, and 5% new martensite in the bulk and the groove sections of the specimen. It should be noted that for each strain path, , the MK-CPFE simulation was repeated five times, and the predicted limit strains using this method is plotted in Fig. 10(a). The FLC2 curve was then obtained by applying the least square fit to these data. Such distribution scheme was used to approximately represent the material microstructure and inhomogeneity in terms of different phase distributions with well-known MK approach, and the results are in better agreement with the scattered experimental limit strains of the QP980. To study the sensitivity of the total number of grain orientations assumed per integration point on FLC curve, additional simulations with 40 grains (represented by 1,824,000 grains) and 10 grains (represented by 456,000 grains) were also performed and compared with predicted FLC2 using 20 grains (Fig. 10(a)). The fitted FLCs for 40 grains and 10 grains are shown in Fig. 10(b) and Fig. 10(c), respectively. These figures also show that compared with the case of using 20 grain orientations, scattering in the data for each strain path, ρ, significantly increases for the case of 10 grains, but it also significantly decreases when 40 grain orientations is used. Increasing the number of grain orientations per integration point will reduce the overall material inhomogeneity and creates less scatter. Fig. 10(d) shows that FLCs predicted by 20 and 40 grains are similar, while that for 10 grains predicts a lower and more conservative FLC curve.

30

(a)

(b)

31

(c)

(d) Fig. 10: Comparison of the predicted FLCs by MK-CPFE (with f0=0.992, ARg = 4 and ARb = 3/5) with experimental data: (a) 20 grains; (b) 40 grains; (c) 10 grains; (d) Comparison of the fitted curves based on the number of grains. 32

Although the incorporation of crystallographic texture and its evolution increases the modeling effort and the computational time for each simulation, it is necessary to consider the phase distribution features in order to improve the prediction of the plastic anisotropy. On the other hand, a realistic distribution of phases has to be considered as well. This can be seen when the simulation results in Fig. 10 indicate that the distribution of constituent phases affect the tensile instability and subsequently the forming strains of the multiphase AHSS.

Fig. 11 shows the effect of initial imperfection factor f 0 on the predicted FLC with the same procedure and material parameters adopted as before for f 0 =0.992 and 20 grains per integration point. As expected, the larger the initial imperfection f 0 , the larger the critical strain for sheet necking. As f 0 increases from 0.992 to 0.994, the FLC0 increases by ~5% with no significant change in the FLC shape. However, FLC0 computed with f 0 =0.996 is on average 15% larger than that predicted with f 0 =0.992. Also, the shape of FLC predicted by f 0 =0.996 is different than those predicted by f 0 =0.992 and f 0 =0.994. Such change in the

shape of FLC can also be observed when using a non-quadratic yield function as f 0 approaches the value of one [30].

Fig. 11: Comparison of the predicted FLCs by MK-CPFE with different imperfection factors. 33

It is well known that for linear strain paths, ρ < 0, the strain localization occurs at an angle inclined to the prescribed major strain rate direction [72]. Hence, the assumption of normal groove to major strain rate direction will overestimate the strain limits for the left-hand side of FLC. Therefore, the left-hand side of FLC was constructed using the limit strain obtained from the time dependent LBF method, as shown in Fig. 12. LBF is employed to determine the major and minor strains at the onset of necking using the simulated hemispherical punch test of a narrow specimen of 20 mm wide in the same way that was adopted by Mohammed et al. [59]. That method showed good results for determining the limit strains for uniaxial and balanced biaxial cases, however, overestimated the experimental results for in-between deformation paths. That overestimation was related to the inhomogeneity effect, which was solved in the current study by incorporating the MK approach to construct the right-hand side of FLC.

Fig. 12: FLC of QP980 predicted by MK-CPFE for the right-hand and LBF-CPFE of the lefthand side.

The simulation methods carried out in the current study successfully predicted the FLC of the 34

QP980 steel. In particular, it is interesting to note that the predicted FLC is in agreement with the experimental measurements, as shown in Fig. 12.

Additional CPFE simulations were performed without considering the groove for the initial imperfection. Based on the observations in Fig. 2, different distribution of the phase volume fraction within a rectangular specimen was considered using the Taylor’s assumption. In the simulations, the same boundary conditions, geometry (ARb=3/5 and ARg=4), and mesh distributions for the rectangular specimen were used as in the MK-CPFE simulation. Instead of having different thickness in the groove section ( f 0 =1.0), different distribution of phase volume fraction was considered as summarized in Table 2. Here, V , V , V , and V

N

denote the volume fraction of ferrite, martensite, retained austenite, and new martensite, respectively. Only the plane strain condition was considered for the simulations and the failure criterion in Eq. (15) was used to determine the forming limit strain. As shown in Fig. 12, the simulation results without the groove predicted similar tensile instability behavior as the result with the groove; i.e., as the volume fraction difference in the groove and bulk sections increases, the inhomogeneity increases. However, the disadvantage of using this method is that it is sensitive to the assumption of inhomogeneous phase distributions, which are not known a priori. This problem becomes exacerbated when the number of material properties to be varied increases. Therefore, from the computational efficiency stand point, it is most optimal to use the model with the groove, while maintaining the same phase volume fractions throughout the specimen. This is because there is only a single parameter, f 0 , that controls the tensile instability. Table 2. Inhomogeneous distribution of phase Groove section

Bulk section

V

V

V

V N

V

V

V

V N

Case 1

50%

40%

5%

5%

40%

50%

5%

5%

Case 2

45%

45%

5%

5%

40%

50%

5%

5%

Case 3

50%

40%

5%

5%

45%

45%

5%

5%

35

0.20

Major strain

0.15

0.10

0.05

0.00 -0.05

Case 1 Case 2 Case 3

0.00

0.05

0.10

0.15

Minor strain

Fig. 13: Forming limit strain of QP980 under the plane strain condition predicted for inhomogeneous distribution of phase volume fractions.

The influence of texture evolution on FLC prediction has already been shown to be important on the necking in single phase metals [43]. In addition to initial texture effect, for multiphase steels, complexity arises due to a difference in the flow characteristics of constituent phases. For example, Fig. 14(b) shows the evolution of 2000 randomly oriented grains per phase at the onset of necking for multiphase QP980 under balanced biaxial tension in the bulk and groove region with f 0 =0.992. As expected, ferrite has more texture intensity and tendency than other phases to accommodate the balanced biaxial deformation mode in the bulk. One may attribute this to the fact that ferrite, beside the high initial volume fraction of 45%, is the softest phase with respect to other three phases. Therefore, the strain heterogeneity in elements that contain high volume fraction of ferrite is much higher than that in other elements in CPFE simulation. Austenite with 5% volume fraction shows a low intensity, and even a little lower intensity can be observed for the harder new martensite when it is compared with the initial texture, as shown in Fig. 14(a). The contribution of each individual phase on the total deformation at the onset of necking was quantified and plotted in Fig. 14(c). For instance, the contribution of ferrite phase is 36

calculated by,

i N grain

j 1

Percent contribution

i j

100 (%)

i N Phase N grain

i 1

j 1

(18)

i j

i where ij is the accumulated shear strain for i-th phase and j-th grain, N grain is the number

of grains for i-th phase, N phase is the number of phases. The ferrite phase shows a little higher plastic strain compared with other phases in the groove and bulk regions. Based on experimental observations, the flow strength of ferrite is lower than that of other phases; therefore, it is expected that plastic deformation initiate in the softer ferrite phase, compared with other harder phases which might even be deforming elastically. From crystal plasticity perspective, however, the plastic deformation could also simultaneously occur in a harder phase, as long as the harder phase is more aligned with the loading direction. For that reason, the plastic strain in the ferrite phase is only slightly larger than that in martensite, which is a harder phase.

Ferrite

(a)

37

Bulk Groove

(b)

38

Austenite New Martensite

Martensite

Percent contribution of each phase to the total deformation

(c) Fig. 14: (a) Initial random orientation; (b) Simulated textures of 2000 orientations at onset of necking represented by (111) stereographic pole figure of an imperfection factor f0=0.992 and balanced biaxial tension (ρ=1); (c) percent contribution of each phase to the total deformation at the onset of necking.

As pointed out before, in the FLC analysis carried out based on MK-CPFE model, the shape of the yield surface for the steel sheet is determined based on the initial texture evolution, and the mechanical properties of constituent phases. Consequently, the individual phase property has one of the most important impacts on the FLC prediction. It can be noticed that ferrite may have an effect on the predicted limit strain and subsequently on FLC more than other phases. This agrees well with DIC measurements when localization in many cases tend to concentrate where ferrite phases are [59].

5.3. FLC validation with the T-shape component CPFE simulation The T-shape stamping was used to evaluate the formability of the QP980 steel sheet under complex forming conditions. The maximum punch stroke without tearing or splitting the sheet was taken as a relative formability index for different test setups. 39

The CPFE simulation of T-shape stamping process was conducted with two different 1.0 mm thick QP980 steel sheets. Failure strains were calculated based on the FLC predicted by the multiphase CPFE model discussed in Section 5.2.

Fig. 15 shows the FE model of the die, punch, blank and blank holder used in the T-shape simulation. Analytical rigid body surfaces were utilized for the die, blank holder and the punch. Blanks were meshed with 0.333 mm × 1 mm elements size (three layers through the thickness) and C3D8R element type from the ABAQUS/Explicit element library [69]. It is well known that computational times increase almost quadratically by increasing element number [3]. Also, reducing the size of the blank element will require additional mesh refinement for the T-shape part, and subsequently increase the computational time required by the microstructure-based CPFE model. Hence, it is important to mention here that multiphase CPFE model was less sensitive to changes made in the element size compared with phenomenological models under large deformation applications [59]. Therefore, additional mesh refinement below 1.0 mm (surface element size) and 0.333 mm (thickness element size) was not considered in this study.

Fig. 15: Schematic diagram for Finite element model of a T-shape component stamping simulation. 40

The Coulomb friction model was used to describe the contact interaction between the rigid body tooling and the deformable blank. A friction coefficient of 0.12 was assumed in the CPFE simulation, as it showed the best fit to the experimental punch force-stroke relationship. Furthermore, since a strain-rate independent material model was assumed in the finite element simulations, and to enhance the calculation speed, mass-scaling was used by setting the minimum step increment time to 10-7 seconds [69]. Stamping simulation of a T-shape was also carried out using the CPFE model with 140 grain orientations per integration point. In addition, the random volume fraction distribution and orientations of the phases were assumed for the sheet metal.

Fig. 16(a) and (b) illustrate the contour plot of the equivalent plastic strain and the corresponding experimental results, respectively, when the punch force reaches the peak value in the T-shape stamping of sample-1, as shown in Fig. 16(c).

(a)

(b)

41

(c)

Fig. 16: CPFE simulation and experimental results of the T-shape stamping sample-1. (a) Equivalent plastic strain distribution based on CPFE model; (b) Experimental final shape results; (c) Comparison of punch force versus punch stroke relationship during the stamping process.

Visual inspection of experimentally stamped T-shape, Fig. 16(b), showed that the part did not fail. It can be seen from simulation results, Fig. 16(a), that plastic strains are highest in the corner areas of the T-shape part where there is severe bending and stretching deformations. However, failure of the T-shape part could not be ascertained by visual inspection of the simulation results alone. Therefore, major and minor strains at the final punch depth, Fig. 16 (c), were calculated from the strain components and plotted on the forming limit diagram (FLD), as shown in Fig. 17.

42

Fig. 17: The minor and major true strain distributions and FLC predicted by CPFE model of T-shape sample-1 at the end of stamping process.

Strains with critical values from multiple regions (elements) with different colors (upper-right corner of Fig. 17) for the simulated T-shape were projected onto the FLD as shown in Fig. 17. According to the simulation results, and compared with the FLC predicted with CPFE model, some of the major and minor strains plotted on the FLD indicate that the stamped T-shape might be experiencing necking. From the experimental perspective, cracks and wrinkles are the type of failures that can be predicted from simulation results using fracture forming limit curve (FFLC) instead of FLC [73]. Hence, the onset of necking cannot be identified just from visual inspection, without experimentally measured forming strains. In addition, the critical strains that crossed the FLC in Fig. 17 may have been due to the slightly larger punch force predicted at the end of the simulation result, as shown in Fig. 16(c). However, overall, the predicted punch force-stroke curve based on the CPFE model and 0.12-friction coefficient is in good agreement with the experimental curve, Fig. 16(c).

The simulation results with the contour of the equivalent plastic strain and the experimental final shape of the T-shape (sample-2) with holes, are shown in Fig. 18(a) and (b), respectively. 43

Here, the simulation results from Fig. 18(a) at ~17.5 mm punch stroke cannot be used for formability assessment because the experimental punch force-stroke curve showed earlier fracture at approximately 14.3 mm punch depth, Fig. 18(c). Therefore, the strains were collected for three punch depths prior to the maximum load occurring at the 14.3 mm punch depth.

(a)

(b)

(c) 44

Fig. 18: CPFE simulation and experimental results of the T-shape stamping sample-2. (a) Equivalent plastic strain distribution based on CPFE model; (b) Experimental final shape results; (c) Comparison of punch force versus punch stroke relationship during the stamping process.

For the safe T-shape component stamping at 12.5 mm punch depth, Fig. 18(c), it was noticed that true strains everywhere in the sheet were less than the critical limit strains as defined by FLC in Fig. 19(a). Also, it was observed that the maximum plastic deformation generated around the holes with no contact surfaces, gradually extended to adjacent regions around the holes as the stamping process progressed to 13.5 mm punch depth, as shown in Fig. 19(b), when the sheet started to experience the onset of necking around the holes. At approximately 14 mm punch depth, the CPFE punch force-stroke curve overestimates the experimental curve. The calculated strains plotted on the FLD in Fig. 19(c) at 14.0 mm punch depth, indicate that the sheet metal is close to fracture since many of the strain points are above the FLC with additional critical strains also occurring at locations away from the holes.

(a) 45

(b)

(c) 46

Fig. 19: The minor and major true strain distributions and FLC predicted by CPFE model of T-shape sample-2 at punch depth (a) 12.5 mm; (b) 13.5 mm and (c) 14.0 mm.

As can be seen from these figures, the CPFE model was able to predict the safe strains, as well as necking strains and failure locations in the sheet at various conditions. However, it can be seen that fracture observed from the experimental test for sample-2, Fig. 18(c), occurred at an earlier punch stroke of 14.3 mm compared with the fracture from the punch force versus punch stroke curves predicted by the CPFE model. The CPFE model in this work was not intended to account for the material behavior beyond the strain localization. In other words, strain rate sensitivity and damage behavior with element deletion were not considered in this study. Also, the extended Voce type hardening rule shown in Eq. (7) converges to the linear hardening rule as the exponent part vanishes with the increasing accumulated shear strain. Therefore, the material model could not accurately predict the necking of the punch force versus punch stroke curves of sample-2.

6. Conclusions In this study, numerical procedure for predicting the forming-limit behavior of steel sheet metals is discussed within the framework of the MK technique using a multiphase computationally efficient rate independent CPFE model. According to all the observations on strain distribution in uniaxial tensile tests, formability tests and metallurgical analysis of the QP980 steel, it was found that the inconsistency of formability is attributed to the microstructural features of the sheet metal. Forming limit strains from the experiments associated with the onset of localized necking within a local area for specified deformation path cannot accurately represent the formability involved during a forming process. CPFE model, which accounts for the grain rotation and evolution of anisotropy, was used for the description of each phase’s mechanical behavior. Inhomogeneity of the sheet metal related to inhomogeneous distribution of phases, random orientations and artificial groove size within the sheet metal showed good prediction of FLC. The accurate prediction of strains at the onset of necking of the T-shape stamped part, offers a promising microstructure-sensitive model that will be highly desirable for the stamping simulation of the third-generation advance high strength steels.

47

Acknowledgements This material is based upon work supported by the Department of Energy under Cooperative Agreement Number DOE DE-EE000597, with United States Automotive Materials Partnership LLC (USAMP).

This report was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor any agency thereof, nor any of their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.

References [1]

D.K. Matlock, J.G. Speer, Third generation of AHSS: microstructure design concepts, 2009. doi:10.1007/978-1-84882-454-6_11.

[2]

M.Y. Demeri, Advanced high-strength Steels, 57 (2013) 1–31. doi:10.1007/978-3-64217665-4.

[3]

A.E. Tekkaya, State-of-the-art of simulation of sheet metal forming, J. Mater. Process. Technol. 103 (2000) 14–22. doi:10.1016/S0924-0136(00)00413-1.

[4]

C. Schwindt, F. Schlosser, M.A. Bertinetti, M. Stout, J.W. Signorelli, Experimental and Visco-Plastic Self-Consistent evaluation of forming limit diagrams for anisotropic sheet metals: An efficient and robust implementation of the M-K model, Int. J. Plast. 73 (2015) 62–99. doi:10.1016/j.ijplas.2015.01.005.

[5]

S.P. Keeler, Determination of Forming Limits in Automotive Stampings, SAE Tech. Pap. 14B (1965) 656–669. doi:10.4271/650535.

[6]

G.M. Goodwin, Application of strain analysis to sheet metal forming in the press shop, SAE Pap. 680093 (1968) 767–774.

[7]

M.J. Serenelli, M.A. Bertinetti, J.W. Signorelli, Study of limit strains for FCC and BCC sheet metal using polycrystal plasticity, Int. J. Solids Struct. 48 (2011) 1109–1119. doi:10.1016/j.ijsolstr.2010.12.013. 48

[8]

K. Janssens, F. Lambert, S. Vanrostenberghe, M. Vermeulen, Statistical evaluation of the uncertainty of experimentally characterised forming limits of sheet steel, J. Mater. Process. Technol. 112 (2001) 174–184. doi:10.1016/S0924-0136(00)00890-6.

[9]

H.W. Swift, Plastic instability under plane stress, J. Mech. Phys. Solids. 1 (1952) 1–18. doi:10.1016/0022-5096(52)90002-1.

[10] R. Hill, On discontinuous plastic states, with special reference to localized necking in thin sheets, J. Mech. Phys. Solids. 1 (1952) 19–30. doi:10.1016/0022-5096(52)900033. [11]

Z. Marciniak, K. Kuczyński, Limit strains in the processes of stretch-forming sheet metal, Int. J. Mech. Sci. 9 (1967) 609–620. doi:10.1016/0020-7403(67)90066-5.

[12] D. Banabic, A review on recent developments of Marciniak-Kuczynski model, Comput. Methods Mater. Sci. (2010) 1–24. [13] F. Barlat, K. Lian, Plastic behavior and stretchability of sheet metals. Part I: A yield function for orthotropic sheets under plane stress conditions, Int. J. Plast. 5 (1989) 51– 66. doi:10.1016/0749-6419(89)90019-3. [14] R. Hill, A Theory of the Yielding and Plastic Flow of Anisotropic Metals, Proc. R. Soc. London A Math. Phys. Eng. Sci. 193 (1948) 281–297. doi:10.1098/rspa.1948.0045. [15] R. Sowerby, J.L. Duncan, Failure in sheet metal in biaxial tension, Int. J. Mech. Sci. 13 (1971) 217–229. doi:10.1016/0020-7403(71)90004-X. [16] H.W. Graf Alejandro, The influence of strain-path changes on formint limit diagrams of Al 6111-T 4, Int. J. Mech. Sci. 36 (1994) 897–910. doi:10.1016/S09240136(02)00311-4. [17] A. Graf, W. Hosford, Effect of Changing Strain Paths on Forming Limit Diagrams of Al 2008-T4, Metall. Trans. a-Physical Metall. Mater. Sci. 24 (1993) 2503–2512. doi:10.1007/BF02646529. [18] W.F. Hosford, A Generalized Isotropic Yield Criterion, J. Appl. Mech. 39 (1972) 607. doi:10.1115/1.3422732. [19] F. Barlat, J.C. Brem, D.J. Lege, K. Chung, Advanced Methods in Materials Processing Defects, Stud. Appl. Mech. 45 (1997) 265–272. doi:10.1016/S0922-5382(97)80028-1. [20] J. Cao, H. Yao, A. Karafillis, M.C. Boyce, Prediction of localized thinning in sheet metal using a general anisotropic yield criterion, Int. J. Plast. 16 (2000) 1105–1129. doi:10.1016/S0749-6419(99)00091-1. [21] A.P. Karafillis, M.C. Boyce, A general anisotropic yield criterion using bounds and a transformation weighting tensor, J. Mech. Phys. Solids. 41 (1993) 1859–1886. doi:10.1016/0022-5096(93)90073-O. [22] A.F. Ávila, E.L.S. Vieira, Proposing a better forming limit diagram prediction: A 49

comparative study, J. Mater. Process. doi:10.1016/S0924-0136(03)00162-6.

Technol.

141

(2003)

101–108.

[23] T.B. Stoughton, X. Zhu, Review of theoretical models of the strain-based FLD and their relevance to the stress-based FLD, Int. J. Plast. 20 (2004) 1463–1486. doi:10.1016/j.ijplas.2003.11.004. [24] S. Soare, D. Banabic, A discussion upon the sensitivity of the MK model to input data, Int. J. Mater. Form. 2 (2009) 503–506. doi:10.1007/s12289-009-0521-x. [25] P. Eyckens, A. Van Bael, P. Van Houtte, Marciniak-Kuczynski type modelling of the effect of Through-Thickness Shear on the forming limits of sheet metal, Int. J. Plast. 25 (2009) 2249–2268. doi:10.1016/j.ijplas.2009.02.002. [26] S. Ahmadi, A.R. Eivani, A. Akbarzadeh, An experimental and theoretical study on the prediction of forming limit diagrams using new BBC yield criteria and M-K analysis, Comput. Mater. Sci. 44 (2009) 1272–1280. doi:10.1016/j.commatsci.2008.08.013. [27] A.A. Zadpoor, J. Sinke, R. Benedictus, Formability prediction of high strength aluminum sheets, Int. J. Plast. 25 (2009) 2269–2297. doi:10.1016/j.ijplas.2009.02.005. [28] P. Eyckens, A. Van Bael, P. Van Houtte, An extended Marciniak-Kuczynski model for anisotropic sheet subjected to monotonic strain paths with through-thickness shear, Int. J. Plast. 27 (2011) 1577–1597. doi:10.1016/j.ijplas.2011.03.008. [29] S. Panich, F. Barlat, V. Uthaisangsuk, S. Suranuntchai, S. Jirathearanat, Experimental and theoretical formability analysis using strain and stress based forming limit diagram for advanced high strength steels, Mater. Des. 51 (2013) 756–766. doi:10.1016/j.matdes.2013.04.080. [30] F. Zhang, J. Chen, J. Chen, Effect of through-thickness normal stress on forming limits under Yld2003 yield criterion and M-K model, Int. J. Mech. Sci. 89 (2014) 92–100. doi:10.1016/j.ijmecsci.2014.08.024. [31] P. Eyckens, H. Mulder, J. Gawad, H. Vegter, D. Roose, T. van den Boogaard, A. Van Bael, P. Van Houtte, The prediction of differential hardening behaviour of steels by multi-scale crystal plasticity modelling, Int. J. Plast. 73 (2015) 1–23. doi:10.1016/j.ijplas.2014.12.004. [32] R. Wagoner, K. Chan, S. Keeler, Forming Limit Diagrams: Concepts, Methods and Applications, 1989. [33] K. Narasimhan, R.H. Wagoner, Finite element modeling simulation of in-plane forming limit diagrams of sheets containing finite defects, Metall. Trans. A. 22 (1991) 2655–2665. doi:10.1007/BF02851359. [34] S.H. Evangelista, J. Lirani, H.A. Al-Qureshi, Implementing a modified MarciniakKuczynski model using the finite element method for the simulation of sheet metal deep drawing, J. Mater. Process. Technol. 130–131 (2002) 135–144. 50

doi:10.1016/S0924-0136(02)00729-X. [35] A.H. Van Den Boogaard, J. Hu, Prediction of sheet necking with shell finite element models, (n.d.). [36] C. Zhang, L. Leotoing, G. Zhao, D. Guines, E. Ragneau, A methodology for evaluating sheet formability combining the tensile test with the M-K model, Mater. Sci. Eng. A. 528 (2010) 480–485. doi:10.1016/j.msea.2010.09.001. [37] A. Srivastava, A.F. Bower, L.G. Hector, J.E. Carsley, L. Zhang, F. Abu-Farha, A multiscale approach to modeling formability of dual-phase steels, Model. Simul. Mater. Sci. Eng. 24 (2016) 25011. doi:10.1088/0965-0393/24/2/025011. [38] E. Cyr, M. Mohammadi, A. Brahme, R.K. Mishra, K. Inal, Modeling the formability of aluminum alloys at elevated temperatures using a new thermo-elasto-viscoplastic crystal plasticity framework, Int. J. Mech. Sci. 128–129 (2017) 312–325. doi:10.1016/j.ijmecsci.2017.05.005. [39] R.J. Asaro, A. Needleman, Overview no. 42 Texture development and strain hardening in rate dependent polycrystals, Acta Metall. 33 (1985) 923–953. doi:10.1016/00016160(85)90188-9. [40] Y. Zhou, K.W. Neale, Predictions of forming limit diagrams using a rate-sensitive crystal plasticity model, Int. J. Mech. Sci. 37 (1995) 1–20. doi:10.1016/00207403(94)00052-L. [41] P.D. Wu, S.R. MacEwen, D.J. Lloyd, K.W. Neale, A mesoscopic approach for predicting sheet metal formability, Model. Simul. Mater. Sci. Eng. 12 (2004) 511–527. doi:10.1088/0965-0393/12/3/011. [42] P.D. Wu, A. Graf, S.R. MacEwen, D.J. Lloyd, M. Jain, K.W. Neale, On forming limit stress diagram analysis, Int. J. Solids Struct. 42 (2005) 2225–2241. doi:10.1016/j.ijsolstr.2004.09.010. [43] P.D. Wu, K.W. Neale, E. Giessen, M. Jain, S.R. MacEwen, a. Makinde, Crystal plasticity forming limit diagram analysis of rolled aluminum sheets, Metall. Mater. Trans. A. 29 (1998) 527–535. doi:10.1007/s11661-998-0134-x. [44] P.D. Wu, K.W. Neale, E. Van Der Giessen, On Crystal Plasticity FLD Analysis, Proc. R. Soc. London A. 453 (1997) 1831–1848. doi:10.1098/rspa.1997.0099. [45] K. Inal, K.W. Neale, a. Aboutajeddine, Forming limit comparisons for FCC and BCC sheets, Int. J. Plast. 21 (2005) 1255–1266. doi:10.1016/j.ijplas.2004.08.001. [46] K. Yoshida, T. Ishizaka, M. Kuroda, S. Ikawa, The effects of texture on formability of aluminum alloy sheets, Acta Mater. 55 (2007) 4499–4506. doi:10.1016/j.actamat.2007.04.014. [47] J.W. Signorelli, M.A. Bertinetti, On the role of constitutive model in the forming limit 51

of FCC sheet metal with cube orientations, Int. J. Mech. Sci. 51 (2009) 473–480. doi:10.1016/j.ijmecsci.2009.04.002. [48] C. John Neil, S.R. Agnew, Crystal plasticity-based forming limit prediction for noncubic metals: Application to Mg alloy AZ31B, Int. J. Plast. 25 (2009) 379–398. doi:10.1016/j.ijplas.2008.05.003. [49] M. Yang, X. Dong, R. Zhou, J. Cao, Crystal plasticity-based forming limit prediction for FCC materials under non-proportional strain-path, Mater. Sci. Eng. A. 527 (2010) 6607–6613. doi:10.1016/j.msea.2010.06.063. [50] H. Wang, P.D. Wu, K.P. Boyle, K.W. Neale, On crystal plasticity formability analysis for magnesium alloy sheets, Int. J. Solids Struct. 48 (2011) 1000–1010. doi:10.1016/j.ijsolstr.2010.12.004. [51] K. Yoshida, M. Kuroda, Comparison of bifurcation and imperfection analyses of localized necking in rate-independent polycrystalline sheets, Int. J. Solids Struct. 49 (2012) 2073–2084. doi:10.1016/j.ijsolstr.2012.04.010. [52] R. Chiba, H. Takeuchi, M. Kuroda, T. Hakoyama, T. Kuwabara, Theoretical and experimental study of forming-limit strain of half-hard AA1100 aluminium alloy sheet, Comput. Mater. Sci. 77 (2013) 61–71. doi:10.1016/j.commatsci.2013.04.025. [53] J.H. Kim, M.G. Lee, D. Kim, F. Barlat, Numerical procedures for predicting localization in sheet metals using crystal plasticity, Comput. Mater. Sci. 72 (2013) 107–115. doi:10.1016/j.commatsci.2013.02.008. [54] M. Mohammadi, A.P. Brahme, R.K. Mishra, K. Inal, Effects of post-necking hardening behavior and equivalent stress-strain curves on the accuracy of M-K based forming limit diagrams, Comput. Mater. Sci. 85 (2014) 316–323. doi:10.1016/j.commatsci.2014.01.017. [55] J. Lévesque, M. Mohammadi, R.K. Mishra, K. Inal, An extended Taylor model to simulate localized deformation phenomena in magnesium alloys, Int. J. Plast. 78 (2015). doi:10.1016/j.ijplas.2015.10.012. [56] C.D. Schwindt, M.A. Bertinetti, L. Iurman, C.A. Rossit, J.W. Signorelli, Numerical study of the effect of martensite plasticity on the forming limits of a dual-phase steel sheet, Int. J. Mater. Form. (2015) 499–517. doi:10.1007/s12289-015-1236-9. [57] L. Wang, J.G. Speer, Quenching and Partitioning Steel Heat Treatment, Metallogr. Microstruct. Anal. 2 (2013) 268–281. doi:10.1007/s13632-013-0082-8. [58] L. Zhang, J. Lin, J. Min, Y. Ye, L. Kang, Formability Evaluation of Sheet Metals Based on Global Strain Distribution, J. Mater. Eng. Perform. 25 (2016) 1–11. doi:10.1007/s11665-016-2054-z. [59] B. Mohammed, T. Park, F. Pourboghrat, J. Hu, R. Esmaeilpour, F. Abu-Farha, Multiscale Crystal Plasticity Modeling of Multiphase Advanced High Strength Steel, 52

Int. J. Solids Struct. (2017). doi:10.1016/j.ijsolstr.2017.05.007. [60] A.R. Zamiri, F. Pourboghrat, A novel yield function for single crystals based on combined constraints optimization, Int. J. Plast. 26 (2010) 731–746. doi:10.1016/j.ijplas.2009.10.004. [61] C. Tome, G.R. Canova, U.F. Kocks, N. Christodoulou, J.J. Jonas, The relation between macroscopic and microscopic strain hardening in F.C.C. polycrystals, Acta Metall. 32 (1984) 1637–1653. doi:10.1016/0001-6160(84)90222-0. [62] A. Zamiri, F. Pourboghrat, F. Barlat, An effective computational algorithm for rateindependent crystal plasticity based on a single crystal yield surface with an application to tube hydroforming, Int. J. Plast. 23 (2007) 1126–1147. doi:10.1016/j.ijplas.2006.10.012. [63] H.J. Bunge, Texture analysis in materials science, Butterworth., 1982. [64] ASTM Int., Standard Test Methods for Tension Testing of Metallic Materials 1, Astm. (2009) 1–27. doi:10.1520/E0008. [65] International Standard ISO 12004-2, Metallic Materials-sheet and Strip Determination of Forming Limit Curves. Part 2: Determination of Forming Limit Curves in the Laboratory. International Organization for Standardization, Geneva, Switzerland., (2008). [66] X. Hu, K.S. Choi, X. Sun, Y. Ren, Y. Wang, Determining Individual Phase Flow Properties in a Quench and Partitioning Steel with In Situ High-Energy X-Ray Diffraction and Multiphase Elasto-Plastic Self-Consistent Method, Metall. Mater. Trans. A Phys. Metall. Mater. Sci. (2016) 1–17. doi:10.1007/s11661-016-3373-2. [67] X.H. Hu, X. Sun, L.G. Hector, Y. Ren, Individual phase constitutive properties of a TRIP-assisted QP980 steel from a combined synchrotron X-ray diffraction and crystal plasticity approach, Acta Mater. 132 (2017) 230–244. doi:10.1016/j.actamat.2017.04.028. [68] Y. Guan, F. Pourboghrat, F. Barlat, Finite element modeling of tube hydroforming of polycrystalline aluminum alloy extrusions, Int. J. Plast. 22 (2006) 2366–2393. doi:10.1016/j.ijplas.2006.04.003. [69] ABAQUS User’s Manual, version 6.14, Hibbit, Karlsson & Sorenson, Providence, RI., (2000). [70] S. Sodjit, V. Uthaisangsuk, Microstructure based prediction of strain hardening behavior of dual phase steels, Mater. Des. 41 (2012) 370–379. doi:10.1016/j.matdes.2012.05.010. [71] J. Lian, F. Barlat, B. Baudelet, Plastic behaviour and stretchability of sheet metals. Part II: Effect of yield surface shape on sheet forming limit, Int. J. Plast. 5 (1989) 131–147. doi:10.1016/0749-6419(89)90026-0. 53

[72] K.W. Hutchinson, J. W., Neale, Sheet Necking II: time independent behaviour, in: Koistinen K. P., Wang N. -M. (Eds.), Mech. Sheet Met. Forming, Plenum, New York. (1978) 127–153. [73] K. Chung, C. Lee, H. Kim, Forming limit criterion for ductile anisotropic sheets as a material property and its deformation path insensitivity, Part II: Boundary value problems, Int. J. Plast. 58 (2014) 35–65. doi:10.1016/j.ijplas.2014.03.014.

54

PII: DOI: Reference:

S0921-5093(18)30526-4 https://doi.org/10.1016/j.msea.2018.04.029 MSA36349

To appear in: Materials Science & Engineering A Received date: 2 January 2018 Revised date: 5 April 2018 Accepted date: 6 April 2018 Cite this article as: Bassam Mohammed, Taejoon Park, Hyunki Kim, Farhang Pourboghrat and Rasoul Esmaeilpour, The Forming Limit Curve for Multiphase Advanced High Strength Steels Based on Crystal Plasticity Finite Element M o d e l i n g , Materials Science & Engineering A, https://doi.org/10.1016/j.msea.2018.04.029 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting galley proof before it is published in its final citable form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.

The Forming Limit Curve for Multiphase Advanced High Strength Steels Based on Crystal Plasticity Finite Element Modeling Bassam Mohammeda, b, Taejoon Parkb, Hyunki Kimb, Farhang Pourboghratb,c *, and Rasoul Esmaeilpourb a

Department of Mechanical Engineering, Michigan State University, 428 S Shaw Ln, East Lansing, MI 48824, United States b

Department of Integrated Systems Engineering, The Ohio State University, 210 Baker Systems, 1971 Neil Avenue, Columbus, OH 43210, United States

c

Department of Mechanical and Aerospace Engineering, The Ohio State University, 201 W 19th Ave, Columbus, OH 43210, United States

April 05, 2018

* Corresponding author. Tel.: +1 (614) 292 3124; E-mail: [email protected]

1

Abstract A computationally efficient rate independent crystal plasticity finite element (CPFE) model was used to predict the forming limit curve (FLC) for a multiphase advanced high strength steel (AHSS). The CPFE model accounts for mechanical properties of the steel phases based on their individual plastic deformation and slip systems. The macroscopic behavior of the polycrystalline aggregate was predicted based on the volume-averaged response of the representative phases, and their volume fraction in the steel sheet. In addition to the random texture distribution assumption for each grain, the volume fractions of various phases were also assumed to be randomly distributed at each integration point. The microstructural inhomogeneity of the material, as well as a geometrical inhomogeneity in the form of a groove region in the specimen, based on the Marciniak-Kuczynski (MK) theory, were considered in the calculation of the FLC using the CPFE model (MK-CPFE). The validity of predicted FLC for quenched and partitioned QP980 steel was confirmed by comparing the results with experimental measurements. The FLC calculated by CPFE model showed that the presence of microstructural inhomogeneity allows for a more realistic prediction of the localized necking phenomenon. Subsequently, the FLC was used to compute the limit strains for the T-shape part stamping process. The limit strains and the punch force-stroke relationship for the T-shape part predicted by the multiphase CPFE model were in good agreement with experimental results.

Keywords: Finite element method, Crystal plasticity, Advanced high strength steel, Forming limit curve, Marciniak–Kuczynski analysis

2

1. Introduction Improved fuel economy, crashworthiness, and a higher stiffness for better drivability all require the application of higher strength materials with good combinations of strength, formability, fatigue resistance, and toughness. As a consequence of the increased demands on steels by automotive manufactures, new products referred to as “advanced high strength steels” (AHSS) have been developed and are now being utilized [1]. AHSS, such as dualphase (DP), complex phase (CP), transformation-induced plasticity (TRIP), and twinning induced plasticity (TWIP) are all multiphase steels which possess a composite microstructure comprised of ferrite, bainite, austenite, and martensite [2]. Consequently, AHSS derive their extraordinary properties from a complex, heterogeneous microstructure and the interactions between different phases.

With the advent of increased application of AHSS in automotive industries, new challenges in the sheet metal forming processes have surfaced, which further spawned new efforts in the fields of experimental, theoretical and numerical modeling. Part of these new initiatives included development and application of new constitutive models, failure criteria and friction models. Also, development of material data needed for the calibration of complex material models became imperative [3]. Understanding how the constituent’s phases in AHSS interact to achieve a desired strength, resistance to localized necking and fracture is particularly challenging. Moreover, volume fraction, grain morphology and micromechanical properties of the constituent phases play an important role during the material selection for automobile components. Therefore, formability assessments of AHSS require an understanding of the effects that material microstructure has on the forming limit strains, as well as on the operating deformation mechanisms.

Failure in sheet metal forming processes are often evaluated based on the onset of localized necking, which is characterized by the forming limit curve (FLC) in the principal strain space. FLC separates the region of uniform sheet deformation from the region of slightly greater deformation, where a local instability or a “neck” occurs [4]. The concept of FLC was pioneered by Keeler [5] for the tension-tension domain of the right hand side of the FLC, and extended by Goodwin [6] to the tension-compression domain. The FLC has been shown to be quite useful in representing the onset of sheet necking, and now is a standard tool for 3

characterizing the material forming behavior and a standard tool to study the formability of sheet metals.

Although the concept of FLC is simple to understand and apply, it has limited application. The actual response and failure of a material during the plastic deformation depends on a large number of coupled effects, making experimental determination of the material failure non trivial and time consuming [7]. In addition, scatter in the experimental data for a given sheet is often so large that researchers sometime question the accuracy and precision with which the FLC has been determined [8]. Experimental determination of the onset of diffuse necking becomes even more important when it comes to multi-phase AHSS sheets, since they are relatively new to stamping engineers.

In view of the continuous push to reduce development costs, considerable efforts must be made to develop microstructure sensitive constitutive models, as well as material instability criteria to assess AHSS sheet metal formability. Early theoretical models proposed by Swift [9] and Hill [10] describe diffuse and localized necking for a homogenous material, respectively. Marciniak and Kuczyński [11] proposed the MK model based on the premise that sheet metals are non-homogeneous from both geometrical and microstructural point of view. According to the MK model, an infinitely long sheet metal contains a local imperfection region (i.e. the grove), which is a band having an initial thickness less than that of the bulk sheet. These authors showed that the presence of such an imperfection could lead to unstable deformation in the grove region, and subsequently result in a localized necking and failure. The MK model has since been one of the most widely applied models for FLC prediction, and well established for predicting sheet metal necking among researchers [12].

In the last five decades, authors have been implementing various yield criteria and hardening rules in the MK model. A common observation is that FLC predictions are very sensitive to the choice of the constitutive model being used [13]. The MK model is frequently used with the quadratic Hill’48 [14] and the von Mises yield functions. However, both models overpredict the limit strains for biaxial paths. Sowerby and Duncan [15] used Hill’48 yield criterion and the Swift type isotropic hardening law [9] to calculate the FLC. They showed that the right-hand side of the FLC increases with an increase in the stain hardening exponent 4

(n-value), and its shape is slightly affected by the normal anisotropic parameter (r-value).

Several non-quadratic yield functions have been developed and subsequently implemented for computational modeling and prediction of limit strains. Graf and Hosford [16,17] predicted the right-hand side of the FLC with the MK analysis using the non-quadratic Hosford yield criterion [18]. The computed FLC was found to increase by increasing the nvalue, and was unaffected by the r-value. The predicted FLC using Hosford yield criterion, although still higher, was in better agreement with the experimental FLC, compared with results obtained with Hill’48 yield criterion. Barlat et al. [19] calculated FLCs for one aluminum and two steel sheets using the Yld94 yield function. Their predictions were in reasonable agreement with experimentally measured FLCs. Cao et al. [20] predicted FLC based on the MK analysis using the K-B yield function developed by Karafillis and Boyce [21], and analyzed the effect of changing the strain-paths on the FLC. An algorithm proposed by Ávila and Vieira [22] was used to predict the right-hand side of the FLC using the methodology proposed by Marciniak and Kuczynski using five different yield criteria. They confirmed that the type of yield criterion used in the analysis strongly influences the FLC. More recently, additional contributions have been made in predicting FLC curves based on the MK analysis using more complex phenomenological models [23–31].

In the MK model, instability is viewed as a process in which the strain state in a small region of the material (i.e., grove) evolves to one of plane strain as deformation proceeds uniformly in the rest of the material (i.e., bulk). In general, this characteristic agrees well with the experimentally observed failures in sheet metals. However, the analytical MK model is based on simplified assumptions, such as the defect is infinite in length and boundary effects are not accounted for. The analytical MK analysis, therefore, implicitly imposes nonphysical boundary conditions by way of assuming uniform minor strains throughout the sample sheet. These two simplifications allow for the derivation of closed form one-dimensional solutions when allowing variations in the field quantities to occur in one direction only [32]. Finite element modeling allows relaxation of these two restricting assumptions by solving for nonuniform internal stresses and strains under prescribed displacement boundary conditions. Therefore, researches have been using phenomenological models and finite element method (FEM) to computationally calculate limit strains within the framework of the MK model 5

(MK-FEM). Narasimhan and Wagoner [33] used the FEM approach to predict the FLC of a sheet specimen with finite defect in the middle of the sheet far from the applied boundary condition. They studied numerous material aspects and their effects on the predicted FLC, as well as validated their results with analytical MK model. However, with an imperfection factor less than 0.98, the strain paths in the groove region showed an earlier deviation from the applied strain path of the bulk and eventually tended to plane strain. This is in contrast with the MK model where the strain path of the groove stays proportional at the beginning and deviation occurs much later. In the MK-FEM, in addition to the imperfection factor, the aspect ratios of the initial groove and the bulk have a significant influence on the rate of strain localization and thus on the predicted FLCs. These effects were not taken into account by some researchers in their MK-FEM, and the imperfection factor was the only parameter used for predicting FLC using different phenomenological models [34–36]. Recently, Srivastava et al. [37] predicted the FLC of two DP steels based on the standard ratedependent, isotropic plasticity model (von Mises), and MK-FEM. The flow behavior of DP steel used for the FLC prediction was calculated with finite element simulation coupled with a microstructure-based crystal plasticity model. In their study, the imperfection factor and the aspect ratio of the groove were only determined from the measurements of the surface roughness of the sheets using a three-dimensional (3D) digital image correlation (DIC) technique. It was found that the prediction of FLC via their method was in good agreement with experimental results only within a limited strain range.

Phenomenological models can describe the effects of initial anisotropy; however, they still have some difficulty accounting for the evolution of the yield surface. In addition, they can be very arduous to calibrate, requiring many experiments and are only valid for monotonic loading. For complex metal forming, the assumption of monotonic loading for predicting limit strains is not adequate [38]. It is well known and widely recognized that the crystallographic texture evolution strongly affects the FLC and the macroscopic anisotropy of polycrystalline sheet metals. Research has shown that the localization of the plastic flow is influenced by deformation-induced textures and anisotropy [39]. Thus, more realistic constitutive models, often involving crystal plasticity, are preferable. These microstructurebased models provide a framework to better understand the relationship between flow localization and the material’s microstructure, and their impacts on forming limits. Issues 6

such as material anisotropy, shape of the yield-surface and crystal orientation can be directly addressed by using a microstructure-based constitutive model.

Zhou and Neale [40] predicted FLCs for annealed aluminum sheet using an analytical polycrystalline model based on Taylor homogenization scheme and the analytical MK model [41]. Many recent studies have employed crystal plasticity models for predicting FLCs for sheet metals based on a single-phase assumption. It is well documented that factors such as the initial imperfection, texture, hardening rate, temperature, and the choice of the constitutive model affect the prediction of FLC [7, 39, 43–57].

The analytical prediction of FLC based on crystal plasticity and MK analysis with more than one phase are scarce in the literature. In a recent study by Schwindt et al. [4,56] the authors investigated formability prediction of DP780 steel with only body centered cubic (BCC) structure (ferrite and martensite). In their study, due to the lack of experimental flow curves for ferrite and martensite, four simulated uniaxial flow curves for these phases were calibrated by matching the experimental flow curve for DP780. Also, because of the high computational cost related to using Visco-Plastic Self-Consistent (VPSC) model in their study, only limited number of orientations were assumed. However, they noted that even when they used thousands of orientations for multiple phases in the steel, the FLCs predicted by MKCPFE model showed, to some extent, sensitivity to the phase distribution.

The typical FLCs for cold rolled QP980, DP780 and DP980 steel sheets have been reported by Wang and Speer [57]. The authors showed that the formability of QP980 is superior to that of DP980 steel, and reaches similar levels as that of DP780. Recently, the formability of three DP980 steels and one QP980 steel was evaluated by Zhang et al. [58] using hemispherical punch tests and DIC technique. Inconsistent and scattered results were observed when they compared the formability of the four AHSS sheets based on the commonly used FLC method. According to their observations of the strain distribution in the hemispherical punch tests and metallurgical analysis of the QP980 steel, the inconsistency and scatter in the formability was attributed to the microstructural features of the sheet metal. They observed that strain valleys occur in the regions with higher martensite volume fraction, and conversely strain peaks occur in regions with a lower volume fraction of martensite. The authors proposed an 7

analytical method based on mathematical expectation and variance to evaluate the formability of sheet metals and correlate them to the global strain distribution observed in DIC. Also, they concluded that the application of traditional formability evaluation methods might not be suitable for the newly developed steel sheets with complex multiphase microstructure. Also, Mohammed et al. [59] numerically studied the formability of QP980 steel using multiphase crystal plasticity simulation of hemispherical punch tests. The authors concluded that the inhomogeneous deformation and formation of strain bands in the steel sheet are related to the inhomogeneous phase distributions, and that it had significant impact on the FLC prediction, and on the scattering observed in the experimentally predicted FLCs.

The most reliable method to numerically predict the FLC for sheet metals is to simulate the hemispherical punch test with similar boundary conditions and specimen sizes used in the experiments. However, given the complex geometry of the hemispherical punch test and specimen shapes, and highly intensive computational time, especially with crystal plasticity finite element method (CPFEM), it was opted in this study to use the simpler rectangular geometry of the specimen used in the MK analysis for the FLC prediction. It was found that the analytical prediction of FLC using MK model in conjunction with crystal plasticity and Taylor homogenization scheme does not accurately predict the forming limits. The main shortcoming of this analytical approach was identified to be its assumption that all crystal orientations exist and evolve at only one material point, and therefore crystal orientation and phases distribution of the specimen cannot be accounted for. In contrast, by using FEM to predict forming limits, multiple integration points with different orientation distributions can be assumed to more accurately represent microstructural properties of the sheet metal. Also, by using FEM to predict FLC, it is possible to impose the more natural boundary conditions, such as displacement or velocity, rather than strains, which are imposed in the analytical model.

Present research focuses on the prediction of the FLC for multiphase AHSS sheet based on the CPFE modeling and the MK theory (MK-CPFE). More specifically, the influence of geometrical and material inhomogeneity on the FLC for AHSS sheet is studied, and some viewpoints about the FLC predictions are expressed based on these two characteristics. The inhomogeneity of various phases within the steel sheet is considered through the crystal 8

plasticity constitutive relationships based on crystallographic slip systems, which not only accounts for the initial elastic–plastic anisotropy, but also for its gradual evolution during the forming process due to the texture evolution. The verification of the accuracy of the adopted method in this study was investigated based on the comparison of predicted and experimental results, in terms of hemispherical punch tests and the stamping of the T-shape component.

2. Crystal Plasticity Constitutive Models The rate-independent crystal plasticity model used in this study was first presented by Zamiri and Pourboghrat [60] for single materials and was recently modified by Mohammed et al. [59] for multiphase metals. A brief summary of the important components of the formulations are presented in this section. The formulations were implemented into the commercial finite element program Abaqus/Explicit via a user material subroutine VUMAT.

2.1. Crystal plasticity yield function In the crystal plasticity model [60], the yield function is defined as:

f (σ, q)

where is the slip system, N

N | σ : P | ln exp 1 1 m y 1

(1)

is the number of slip systems, y is the critical resolved

shear stress (CRSS), ρ is a parameter to determine the closeness to the condition,

| σ : P | y , and m is a parameter for a flexible yield function shape. Also, Pα is a matrix of the Schmid tensor and I describes the orientation of a slip system, defined as:

1 P [m n (m n )T ] 2

(2)

where n is a unit vector representing the normal to the slip plane, and m is a unit vector denoting the slip direction. The plastic deformation gradient can be expressed as: N

DP P 1

9

(3)

where are the shear slip rates. The spin tensor, which represents the material rotation due to slip, can be expressed as: N

P ω

(4)

1

where ω matrix is the anti-symmetric part of P , defined as:

1 ω [m n (m n )T ] 2

(5)

The slip rate on any slip system can be expressed by: σ : P exp 1 y m y σ:P N m exp 1 m y 1

sgn(σ : P )

(6)

where represents the index of summation for slip systems, m and are material parameters that control the shape of the single-crystal yield surface, which have been shown to have a direct relationship with the stacking fault energy of the material. 2.2. Hardening model In order to define the resistance against shear stress, an extended Voce type strain hardening type [61] was used:

0 1

y () 0 1 1 1 exp

(7)

where is the total accumulated shear strain over the entire deformation, and y is the critical resolved shear stress on the slip system as a function of . The initial yielding is 10

characterized by 0 , and 0 is the hardening rate, while the asymptotic hardening is characterized by 1

and 1 . The extended Voce model represents the exponential

hardening which consists of the initial critical resolved shear stress, 0 , and the work hardening rate, 0 . The excess stress 1 can be obtained before the critical resolved shear stress reaches saturation where the sum of 0 and 1 is the saturation stress at which the work hardening rate approaches zero. The 1 represents a constant work hardening rate for the linear hardening part of extended Voce-law. The total accumulated shear strain on all slip systems , can be defined as:

N 1

dt

(8)

2.3. Homogenization method In the present study, the Taylor type homogenization was used for the calculation of the homogenized stress in case of multiple grains were considered for each integration point in the finite element simulations. According to the Taylor model, which is an upper bound model, each grain of the polycrystal aggregate undergoes the same deformation and deformation rate. Therefore, the deformation gradient in Eq. (3) in all grains are the same and equal to the overall deformation gradient.

By assuming that grains have the same volume V c for simplicity, the homogenized stress,

σ , can be calculated from the crystal stress σ c : σ

Vc V

σ

c

c

1 M

σ

c

(9)

c

where V is the total volume of grains, and M is the number of grains [62]. For multiphase materials, Eq. (9) can be rewritten in the form:

1 σ fi i 1 Mi

11

σ c

i c

(10)

where fi is the volume fraction of each phase. Eq. (10) is then used in the explicit algorithm to calculate the macroscopic stress tensor from the crystal stress tensors for all phases. 2.4. Crystal orientation For the material texture representation, the three Euler angles 1 , and 2 that are defined based on Bunge convention to define the orientation of any crystal with respect to the material coordinate system is used [63]. Based on the Bunge system, the orientation of a crystal can be defined by the three Euler angles to create a rotation tensor Q as, sin 1 sin 2 cos 1 sin 2 cos sin 2 sin cos 1 cos 2 sin 1 sin 2 cos Q(1 , , 2 ) cos 1 cos 2 sin 1 sin 2 cos sin 1 sin 2 cos 1 cos 2 cos cos 2 sin sin 1 sin cos 1 sin cos

(11)

3. Material Characterization In this study, to verify the accuracy of the proposed methodology for predicting FLC based on CPFE, numerically generated results were validated against various experiments conducted with the QP980 sheets. The strain hardening characteristics of the steel were determined using uniaxial tension tests performed along the rolling direction. Experimental results from a hemispherical punch test were also compared with numerically predicted results to verify the accuracy of the proposed methods. The tensile and hemispherical punch test procedures have been discussed in details in Mohammed et al. [59], for the sake of completeness, these experimental procedures and relevant results for the QP980 are summarized briefly in the present work. Also, this section summarizes the properties of the QP980 used in this work as well as the calibrated hardening parameters with the uniaxial flow curve for parent QP980 and its constituent’s phases.

3.1. Mechanical and microstructure behavior The uniaxial tensile behavior of the QP980 steel sheet was measured using a universal tensile testing machine. ASTM E8 [64] standard tensile specimens were used to measure stressstrain curves in the rolling direction (RD), diagonal direction (DD), and transverse direction (TD) (or 0o,45o, and 90o to RD, respectively) at the nominal strain rate of 0.002 s-1. For strain 12

measurements, a 3D system DIC technique ARAMIS 5M was used to monitor the deformation of the test specimens. The uniaxial tensile stress–strain curves for the QP980 at room temperature with different alignment to the RD are shown in Fig. 1. This figure also shows the QP980 sheet’s microstructure inhomogeneity as bands appearing on its surface detected by DIC along diagonal and transverse directions at 4% strain.

Fig. 1: Uniaxial tensile stress–strain curves for the QP980 sheet steel with loading axis aligned parallel, diagonal (DD) and normal (TD) to the rolling direction (RD).

The optical micrographs taken from the middle of the sheet for cross sections perpendicular to the TD and perpendicular to the RD are shown in Fig. 2(a) and (b), respectively. It can be seen that the spatial distribution of martensite (dark regions) is not uniform. Such martensite morphology and inhomogeneous distribution had a significant influence on the accumulation of strains in soft phases such as ferrite (light regions) and subsequently on FLC prediction.

13

(a)

(b)

Fig. 2: Micrographs taken from cross sections of the QP980 sheet showing the size of the martensite band (dark regions) in the microstructure. (a) perpendicular to the transverse direction (TD) and (b) perpendicular to the rolling direction (RD).

3.2. Hemispherical punch test The Hemispherical punch tests were conducted at room temperature to study the formability of QP980. Different blanks with varying width ranging from 20 mm up to 180 mm, and a 1.0 mm gauge thickness were stretched by the hydraulic displacement of the punch at a constant tool velocity of 1 mm/s [65]. A 3D DIC system was employed to measure strain histories on the blank’s surface. The formability of the QP980 was then evaluated based on FLC which was constructed by using the linear best fitting (LBF) method [59].

3.3. T-Shape component stamping The T-shape stamping was used in the present research to validate proposed methods for predicting the FLC based on multiphase CPFE model. This test was speciﬁcally designed to closely replicate actual forming conditions experienced by the sheet metal during the continuous stamping production. The T-shape stamping of 1.0 mm thickness QP980 steel sheets were carried out using Interlaken Servo-Press 150 system. Fig. 3(a) shows the tooling and the experimental setup, and Fig. 3(b) shows two different blanks used in the experiments: with and without holes. The formability of QP980 steel was investigated under a constant binder load of 20.0 Ton, and a punch speed of 0.1 mm/s. The T-shape stamping process took place in two steps: first a constant binder load was applied on the blank, and then the T-shape was formed under the actions of die and punch.

14

(a)

(b) Fig. 3: (a) The sheet metal stamping press tool components setup; (b) Dimensional characteristics of the specimens used in the T-shape experiments.

3.4. Calibration of the material parameters 3.4.1. Phenomenological model The von Mises yield function with isotropic hardening was used in this study to represent the plastic deformation of QP980 steel sheet. The properties of the von Mises yield function were determined using the uniaxial tensile data along the RD. The isotropic elastic constants used for the QP980 steel sheet were determined as C11 =269.23 GPa, C12 =115.38 GPa, and C44 =76.92 GPa. Uniaxial tension data along the RD was considered as the reference state for characterization of the Swift type isotropic hardening law [9]:

15

K ( 0 )n

(12)

where and are the effective stress and equivalent plastic strain, respectively, while K,

0 and n are the hardening coefficients. The hardening coefficients were determined using the least square method based on the experimental true stress-plastic strain curve along the RD. The following material parameters have been obtained: K = 1413.64 MPa, 0 = 2.1192×10-3 and n = 0.099. 3.4.2. Crystal plasticity model The material properties used to generate the simulated stress–strain curves of constituent phases are obtained by curve fitting uniaxial stress–strain simulations by crystal plasticity to experimental results. The experimental data from the in-situ high energy X-ray diffraction (HEXRD) test were used for the calibration of the parameters of the hardening model. These hardening parameters were fitted to each phase using the calibration method detailed by Mohammed et al. [59] and are listed in Table 1. [66,67]

Table 1. Material parameters for the CPFE model composed of four phases in QP980 steel (unit: MPa)

Martensite

0 348 487

1 130 55

0 1100 1994

1 117 185

Austenite

600

2

1600

550

New Martensite

496

39

2200

1788

Phase Ferrite

Fig. 4 shows the comparison between the experimental stress-strain curves for individual phases with the curves predicted by the CPFE model with 60 grain orientations assumed per gauss point for individual phases. Fig. 4 also shows the comparison between predicted and experimental macroscopic stress-strain curve for QP980 steel.

16

Fig. 4: Comparison of the experimental strain–stress curve with the CPFE model with 60 grain orientations assumed for each constituent phase and the QP980.

The effect of changing the number of grain orientations assumed per integration point on computed stress-strain curves for the case of uniaxial tensile test is shown in Fig. 5. It was also shown by others that increasing or reducing the number of grain orientations per integration point will have little impact on the macroscopic stress-strain curve [62,68].

17

Fig. 5: Comparison of the experimental strain–stress curve with the CPFE model in terms of the number of grain orientations assumed per integration point.

4. FLC Determination Procedures Based on Finite Element Simulation In this section, a multi-scale computational framework based on MK theory [11] and CPFE model (i.e., MK-CPFE) is developed to predict FLC for multiphase steel sheets. Similar to MK theory, the right-hand side of FLC is determined with CPFE using a rectangular specimen with a groove in the mid-section. To determine the appropriate geometry of the rectangular specimen, however, a number of finite element simulations were first performed with von Mises yield function (i.e., MK-FEM) to study the sensitivity of predicted FLC to geometrical parameters discussed in Section 4.1. Finally, the left-hand side of FLC was determined with only one point obtained from the CPFE simulation of the uniaxial deformation of a narrow specimen with a hemispherical punch test, and the LBF method [59] . 4.1. The finite element procedure and the failure criteria In the MK model, an imperfection, or a groove, is assumed to exist initially in the sheet metal as illustrated in Fig. 6(a). In real materials, however, numerous imperfections are present at arbitrary angles, and therefore, imperfections aligned at different angles should be considered for obtaining more accurate results. However, due to the inhomogeneous phase distributions in the QP980 sheet (Fig. 1), the localized strain and fracture were mostly observed to take place along the RD in the experiments [59]. Therefore, for the sake of simplicity and computational cost reduction, only an imperfection parallel to the RD, which corresponds to the x1 axis in Fig. 6(a), was considered for the calculation of the right-side of FLC based on the MK-FEM model.

In this study, a sheet specimen with the bulk thickness of t0b , width (dimension along x1) of 2W, and a total length (dimension along x2) of 2L was considered, as shown in Fig. 6(a). The Cartesian tensor notation was used, and the origin of the coordinate system was taken to be at the center of the specimen (i.e. sheet specimen was oriented so that the x1, x2, and x3-axes were parallel to the RD, TD, and normal direction (ND) of the sheet material, respectively). In order to reduce the computational cost, symmetric boundary conditions along x1 and x2 18

axes were assumed for regions 0 x1 W and 0 x2 L , so that only one quarter of the sheet specimen was needed for computational modeling, as shown in Fig. 6(a).

The commercial software MATLAB was used to generate different dimensions for groove and bulk regions. The dimensional values were then used in the mesh generation, creation of a FE model, and subsequent simulations with the commercial software ABAQUS [69]. Solid elements were used for FE simulations as illustrated in Fig. 6(a), with fine symmetric mesh (0.05 mm × 0.05 mm elements) in the groove region. A gradual increase in the mesh size in the bulk region, along x2 direction from 0.1 mm to 0.4 mm, was assumed in order to increase computational efficiency. To have a smooth transition of strains between the bulk and groove, a transition region with one element (0.1 mm thickness) was adopted, as shown in Fig. 6(b). The generated strains in the transition region were neglected in the analysis since they did not represent either the bulk or the groove region.

In all the MK-FEM simulations, the nominal thickness of the specimen in the bulk region was assumed to be t0b =1.0 mm, which corresponds to the measured average thickness of the QP980 sheets used in all the experiments. Also, the specimen width (W) was fixed to 3 mm length. The other two in-plane dimensions, Lg and Lb were iteratively adjusted until the best values for the bulk and groove aspect ratios (ARb and ARg) were found, such that the MKFEM predicted FLC matched the FLC calculated by analytical MK model. The selected parameters were chosen such that a direct comparison with the analytical MK model could be made. Therefore, the following three-groove aspect ratios (ARg) were considered, 4, 6, and 7.5, in the MK-FEM simulations. In addition, three aspect ratios for the bulk region were assumed for calibration. To determine the thickness of the groove region, it was gradually reduced until strain localization occurred inside of the imperfection area. The initial thickness of the groove region is given by: t0g f 0 t0b

19

(13)

where f 0 is the inhomogeneity factor, t0g and t0b are initial thicknesses of the groove and bulk, respectively. The sheet specimen was deformed under in-plane biaxial straining by prescribing the displacements d1 and d2. Therefore, the state of biaxial stretching was imposed as following:

1 2

0 1

(14)

where is the strain ratio corresponding to the deformation path, 1 and 2 are strains caused by imposing displacements d1 and d2 on planes A1 and A2, respectively, as shown in Fig. 6(a) and (b). It is important to mention that by imposing uniform displacements d1 and d2 in the FEA, only proportional engineering strains will be developed, and not the proportional true strains needed to construct FLC. To get around this problem, non-uniform displacements d1 and d2 had to be generated analytically first, and then imposed in the MK-FEM simulations to generate proportional true strains throughout the deformation. Fig. 6(c) visually shows the difference in proportionality between engineering and true quantities generated by assuming that 0.5 in engineering quantities (blue line). From the non-proportional engineering strain history, true strain history was converted and illustrated in red line, which can clearly show that the proportionality in true strains were maintained.

20

21

(c) Fig. 6: (a) Schematic of the undeformed finite element mesh, representing full and one quarter of sheet blank. The sheet blank is subjected to biaxial straining by applying displacements, d1 and d2 and symmetric boundary conditions; (b) Schematic of a sheet characteristics and dimensions; (c) A comparison between the engineering and true strains histories on the prediction of FLC for 0.5 .

During initial stages of the biaxial stretching of the sheet simulations, the sheet deformed uniformly in both the bulk and groove regions. However, as plastic deformations increased, a strain gradient developed and strains inside the groove region grew much faster than in the bulk region, resulting in a localized neck. To predict the limit strains from the groove region corresponding to the formation of a neck, the failure criterion was used. The FLC was then constructed by repeating the simulations for several different strain paths (i.e., 0 1 ), and plotting the principal strains in the bulk region once the assumed failure criterion was reached. In this study, the failure criterion was based on the onset of necking, identified as:

22g b 22

22

10

(15)

where,

g 22

1 Ng

22b

1 Nb

Ng

n 1

Nb

g n 22

(16)

n 1

b n 22

(17)

The sum of 22 in equations (16) and (17) is taken over all elements within groove and bulk regions, respectively. Ng and Nb are the total number of elements in groove and bulk regions, respectively.

The value of

22b

at the onset of necking in Eq. (17) will be referred to as the ‘major strain’

and the corresponding value of

11b

b (analogous to 22

in Eq. (17)) will be referred to as

the ‘minor strain’ for construction of FLCs. To predict FLCs of the steel sheet based on von-Mises model, FE simulations of in-plane biaxial straining of the steel sheet specimen characterized by varying aspect ratios of the groove and the bulk were carried out. These simulations used the calibrated hardening parameters based on the Swift type model shown in Eq. (12).

4.2. Crystal plasticity finite element procedure for phases implementation AHSSs have a considerably complicated microstructure, and their mechanical behavior cannot be explained by simple models, such as those proposed for metal-matrix composites [70]. Thus, applying a more complex constitutive model, such as crystal plasticity that accounts for microstructural properties, is required. However, when simulating complex deformation of steels, some simplifying assumptions must be made about texture to keep the CPFEM computational costs reasonably low, without sacrificing accuracy.

The experimental observations of the QP980 steel sheet revealed that this material is comprised of 44±2% by volume of martensite, ~8–10% by volume of retained austenite, and the rest ferrite. Using this information, the overall microstructure of QP980 steel sheet was 23

modeled with CPFE based on 45% ferrite, 45% pre-existing martensite, 5% retained austenite, and 5% transformed martensite. In the absence of an austenite to martensite phase transformation model in CPFE, it was assumed that a 5% new (transformed) martensite exists in the undeformed sheet from the beginning of deformation. However, in the real material, the volume faction of the new martensite evolves with increasing plastic strain. The assumption of having 5% new martensite available from the beginning of the deformation will not affect the material behavior in a significant way, since the newly transformed martensite will have low volume fraction compared to many TRIP steels.

Based on the EBSD data presented for the QP980 steel sheet in [59], it was concluded that assuming a random crystallographic orientation for aggregate grains is reasonable. Also, the slip systems used in the CPFEM for the deformation of BCC crystals (ferrite, old martensite, and new martensite) were (12 {110} and 12 {112} slip systems), while the following 12 slip systems ({111} slip systems) were considered for the FCC crystal (retained austenite). Finally, in this study, it was attempted to model the multiphase QP980 steel in such a way to represent its real microstructure and inhomogeneities. Therefore, a random phase distribution was assumed at each integration point, but the total distribution for each phase in the sheet was maintained at 45% ferrite, 45% old martensite, 5% austenite, and 5% new martensite. In other words, not every FE integration point had the same volume fraction of each phase. This scheme was adopted for prediction of FLC with the CPFE model, and for the simulation of the T-shape stamping. 5. Results and Discussion 5.1. Aspects ratios calibration with analytical MK model Forming limits of the steel sheet under biaxial stretching were calculated using the framework described in Section 4.1. The calculated forming limits based on von Mises and MK-FEM were compared with the calculated data based on the analytical MK model. The predicted FLCs based on changing the aspect ratio of the groove, ARg, and imperfection factor, f 0 , for a fixed bulk aspect ratio of ARb 3 5 , are shown in Fig. 7(a)-(c). 24

(a)

(b)

25

(c) Fig. 7: Comparison between the predicted FLCs based on analytical MK model and MKFEM for different groove aspect ratios with fixed bulk aspect ratio ( ARb =3/5); (a) f 0 =0.992; (b) f 0 =0.994; (c) f 0 =0.996.

From the comparison of the relative positions of the different curves in Fig. 7, it is apparent that the size of the groove as characterized by the ARg , for a given f 0 , influences the level of the FLC. The conclusion is that a defect (groove) can cause a strain localization that is controlled by both f 0 and its aspect ratio ( ARg ) . Compared with the analytical MK model, the MK-FEM model overestimates the magnitude of FLC0 (plane strain) as the assumed groove aspect ratio becomes larger than 4. For example, as shown in Fig. 7(c), for f 0 =0.996 and ARg =7.5, the FLC0 computed by FEM is on average 13% larger than those computed by the analytical MK model. This is an expected result as the assumed analytical MK defect is more severe for a given sheet thickness than the defect assumed in the MK-FEM model, and hence the plastic deformation localizes faster. Therefore, the ARg for the MK-FEM model must be adjusted to match the specified FLC0 for a given material. 26

The FLC calculated by the MK-FEM model with the ARb 1.0 , predicts forming strains that are slightly larger than those predicted by the analytical MK model for ρ less than 0.5, as shown in Fig. 8. Less sensitivity was noticed when the values of ARb reduced to 3/5 and 3/7.

Fig. 8: Bulk’s aspect ratio (ARb) effects on the of predicted MK-FEM forming limit curve for fixed groove aspect ratio (ARg=4) and imperfection factor (f0=0.992).

The effect of the aspect ratios on FLC predictions can be summarized as follows; increasing the value of ARg increases the values of the limit strains, whereas the values of the limit strains decrease when the values of ARb increases. However, the values of the limit strains are less sensitive to the changes in ARb compared with the changes in ARg values. The shape of analytical MK and MK-FEM FLCs are nearly identical for strain paths in the range of 0 ≤ ≤ 0.5, and FLC0, except for strain paths in the range of

0.6 ≤ ≤ 1, as

shown in Fig. 7. The comparison between various strain paths in groove and bulk regions is also shown in Fig. 9 for five different cases. The respective strain paths for the groove and 27

bulk calculated from the analytical MK model generally match the strains paths predicted by MK-FEM. However, small deviation can be observed in the cases of > 0.6.

Fig. 9: Comparison of the predicted MK-FEM and analytical MK model strain paths for an imperfection factor f0=0.992. As mentioned, the deformation behavior in the groove and the adjacent bulk with MK-FEM and analytical MK model is different because of the nonuniformity introduced by the presence of finite dimensions of groove and bulk with MK-FEM. Therefore, all limit strains from MK-FEM are not expected to have similar values to those predicted by analytical MK model due to the uniqueness of each model. Hence, the calibration method with analytical MK model was proposed here to find the best parameters that give approximate limit strains to that calculated by MK-FEM, and subsequently avoid choosing arbitrary dimensions that may affect the FLC prediction by adopting different constitutive models.

As expected, the FLCs calculated by MK models (analytical MK and MK-FEM), using von Mises and Swift type model for QP980 showed low plane strain (FLC0) value, and high balanced biaxial strain limits, which is inconsistent with what was observed from 28

experimental results of QP980 steel [57–59]. It should be mentioned that FLC predicted by MK models (analytical MK and MK-FEM) is the combined result of the assumed failure model and the consitututive model that describes material properties and behaviour under plastic deformation. In the next section, it will be shown that by adopting a more sophisticated material model (crystal plasticity), but the same failure model described in Section 4.1. , more accurate results that better fit experimental measurments can be obtained.

5.2. FLC prediction based on MK-CPFE It is well known that a slight change in the shape of the yield surface for a sheet metal can have a rather large effect on predicted FLC [71]. In the MK-CPFE forming limit curve analysis carried out here, beside the mechanical properties of various phases, the shape of the ‘yield surface’ for the sheet metal is specified by the assumed initial texture, as well as its evolution.

The MK analysis predicts the FLC based on the growth of an initial imperfection factor f 0 . However, the strength of the imperfection cannot be directly measured by physical experiments. Thus, it is possible to predict the experimentally observed FLC0 by a suitable choice of the f 0 . In other words, since f 0 has no physical meaning, it is simply a fitting parameter that allows a model to be calibrated by matching the experimentally measured FLC0. Here, the lowest initial imperfection factor ( f 0 =0.992) and the initial aspects ratios of ARg = 4 and ARb = 3/5 were chosen for the FLC prediction based on MK-CPFE. These

values showed the best fit for the lowest strain limit in plane strain condition (FLC0) of the QP980 steel.

The initial texture (represented by 912,000 grains) with 20 grains per integration point was employed in the FLC simulations, as shown in Fig. 10(a). The orientations and volume fractions of phases were distributed randomly in all integration points. Fig. 10(a) shows two different strategies to model FLC based on random distribution of phases. FLC1 was predicted by using the same randomly generated volume fraction and orientation distributions in all integration points for all strain paths ( 0 1 ). On the other hand, FLC2 was predicted by using different randomly generated volume fraction and orientation distributions 29

in all integration points for all strain paths ( 0 1 ). In the second method, the material subroutine (multiphase CPFE-VUMAT) randomly generated a new volume fraction of phases and orientation distributions for each simulation run. In all the simulations, however, the volume fraction of phases were kept at 45% ferrite, 45% old martensite, 5% austenite, and 5% new martensite in the bulk and the groove sections of the specimen. It should be noted that for each strain path, , the MK-CPFE simulation was repeated five times, and the predicted limit strains using this method is plotted in Fig. 10(a). The FLC2 curve was then obtained by applying the least square fit to these data. Such distribution scheme was used to approximately represent the material microstructure and inhomogeneity in terms of different phase distributions with well-known MK approach, and the results are in better agreement with the scattered experimental limit strains of the QP980. To study the sensitivity of the total number of grain orientations assumed per integration point on FLC curve, additional simulations with 40 grains (represented by 1,824,000 grains) and 10 grains (represented by 456,000 grains) were also performed and compared with predicted FLC2 using 20 grains (Fig. 10(a)). The fitted FLCs for 40 grains and 10 grains are shown in Fig. 10(b) and Fig. 10(c), respectively. These figures also show that compared with the case of using 20 grain orientations, scattering in the data for each strain path, ρ, significantly increases for the case of 10 grains, but it also significantly decreases when 40 grain orientations is used. Increasing the number of grain orientations per integration point will reduce the overall material inhomogeneity and creates less scatter. Fig. 10(d) shows that FLCs predicted by 20 and 40 grains are similar, while that for 10 grains predicts a lower and more conservative FLC curve.

30

(a)

(b)

31

(c)

(d) Fig. 10: Comparison of the predicted FLCs by MK-CPFE (with f0=0.992, ARg = 4 and ARb = 3/5) with experimental data: (a) 20 grains; (b) 40 grains; (c) 10 grains; (d) Comparison of the fitted curves based on the number of grains. 32

Although the incorporation of crystallographic texture and its evolution increases the modeling effort and the computational time for each simulation, it is necessary to consider the phase distribution features in order to improve the prediction of the plastic anisotropy. On the other hand, a realistic distribution of phases has to be considered as well. This can be seen when the simulation results in Fig. 10 indicate that the distribution of constituent phases affect the tensile instability and subsequently the forming strains of the multiphase AHSS.

Fig. 11 shows the effect of initial imperfection factor f 0 on the predicted FLC with the same procedure and material parameters adopted as before for f 0 =0.992 and 20 grains per integration point. As expected, the larger the initial imperfection f 0 , the larger the critical strain for sheet necking. As f 0 increases from 0.992 to 0.994, the FLC0 increases by ~5% with no significant change in the FLC shape. However, FLC0 computed with f 0 =0.996 is on average 15% larger than that predicted with f 0 =0.992. Also, the shape of FLC predicted by f 0 =0.996 is different than those predicted by f 0 =0.992 and f 0 =0.994. Such change in the

shape of FLC can also be observed when using a non-quadratic yield function as f 0 approaches the value of one [30].

Fig. 11: Comparison of the predicted FLCs by MK-CPFE with different imperfection factors. 33

It is well known that for linear strain paths, ρ < 0, the strain localization occurs at an angle inclined to the prescribed major strain rate direction [72]. Hence, the assumption of normal groove to major strain rate direction will overestimate the strain limits for the left-hand side of FLC. Therefore, the left-hand side of FLC was constructed using the limit strain obtained from the time dependent LBF method, as shown in Fig. 12. LBF is employed to determine the major and minor strains at the onset of necking using the simulated hemispherical punch test of a narrow specimen of 20 mm wide in the same way that was adopted by Mohammed et al. [59]. That method showed good results for determining the limit strains for uniaxial and balanced biaxial cases, however, overestimated the experimental results for in-between deformation paths. That overestimation was related to the inhomogeneity effect, which was solved in the current study by incorporating the MK approach to construct the right-hand side of FLC.

Fig. 12: FLC of QP980 predicted by MK-CPFE for the right-hand and LBF-CPFE of the lefthand side.

The simulation methods carried out in the current study successfully predicted the FLC of the 34

QP980 steel. In particular, it is interesting to note that the predicted FLC is in agreement with the experimental measurements, as shown in Fig. 12.

Additional CPFE simulations were performed without considering the groove for the initial imperfection. Based on the observations in Fig. 2, different distribution of the phase volume fraction within a rectangular specimen was considered using the Taylor’s assumption. In the simulations, the same boundary conditions, geometry (ARb=3/5 and ARg=4), and mesh distributions for the rectangular specimen were used as in the MK-CPFE simulation. Instead of having different thickness in the groove section ( f 0 =1.0), different distribution of phase volume fraction was considered as summarized in Table 2. Here, V , V , V , and V

N

denote the volume fraction of ferrite, martensite, retained austenite, and new martensite, respectively. Only the plane strain condition was considered for the simulations and the failure criterion in Eq. (15) was used to determine the forming limit strain. As shown in Fig. 12, the simulation results without the groove predicted similar tensile instability behavior as the result with the groove; i.e., as the volume fraction difference in the groove and bulk sections increases, the inhomogeneity increases. However, the disadvantage of using this method is that it is sensitive to the assumption of inhomogeneous phase distributions, which are not known a priori. This problem becomes exacerbated when the number of material properties to be varied increases. Therefore, from the computational efficiency stand point, it is most optimal to use the model with the groove, while maintaining the same phase volume fractions throughout the specimen. This is because there is only a single parameter, f 0 , that controls the tensile instability. Table 2. Inhomogeneous distribution of phase Groove section

Bulk section

V

V

V

V N

V

V

V

V N

Case 1

50%

40%

5%

5%

40%

50%

5%

5%

Case 2

45%

45%

5%

5%

40%

50%

5%

5%

Case 3

50%

40%

5%

5%

45%

45%

5%

5%

35

0.20

Major strain

0.15

0.10

0.05

0.00 -0.05

Case 1 Case 2 Case 3

0.00

0.05

0.10

0.15

Minor strain

Fig. 13: Forming limit strain of QP980 under the plane strain condition predicted for inhomogeneous distribution of phase volume fractions.

The influence of texture evolution on FLC prediction has already been shown to be important on the necking in single phase metals [43]. In addition to initial texture effect, for multiphase steels, complexity arises due to a difference in the flow characteristics of constituent phases. For example, Fig. 14(b) shows the evolution of 2000 randomly oriented grains per phase at the onset of necking for multiphase QP980 under balanced biaxial tension in the bulk and groove region with f 0 =0.992. As expected, ferrite has more texture intensity and tendency than other phases to accommodate the balanced biaxial deformation mode in the bulk. One may attribute this to the fact that ferrite, beside the high initial volume fraction of 45%, is the softest phase with respect to other three phases. Therefore, the strain heterogeneity in elements that contain high volume fraction of ferrite is much higher than that in other elements in CPFE simulation. Austenite with 5% volume fraction shows a low intensity, and even a little lower intensity can be observed for the harder new martensite when it is compared with the initial texture, as shown in Fig. 14(a). The contribution of each individual phase on the total deformation at the onset of necking was quantified and plotted in Fig. 14(c). For instance, the contribution of ferrite phase is 36

calculated by,

i N grain

j 1

Percent contribution

i j

100 (%)

i N Phase N grain

i 1

j 1

(18)

i j

i where ij is the accumulated shear strain for i-th phase and j-th grain, N grain is the number

of grains for i-th phase, N phase is the number of phases. The ferrite phase shows a little higher plastic strain compared with other phases in the groove and bulk regions. Based on experimental observations, the flow strength of ferrite is lower than that of other phases; therefore, it is expected that plastic deformation initiate in the softer ferrite phase, compared with other harder phases which might even be deforming elastically. From crystal plasticity perspective, however, the plastic deformation could also simultaneously occur in a harder phase, as long as the harder phase is more aligned with the loading direction. For that reason, the plastic strain in the ferrite phase is only slightly larger than that in martensite, which is a harder phase.

Ferrite

(a)

37

Bulk Groove

(b)

38

Austenite New Martensite

Martensite

Percent contribution of each phase to the total deformation

(c) Fig. 14: (a) Initial random orientation; (b) Simulated textures of 2000 orientations at onset of necking represented by (111) stereographic pole figure of an imperfection factor f0=0.992 and balanced biaxial tension (ρ=1); (c) percent contribution of each phase to the total deformation at the onset of necking.

As pointed out before, in the FLC analysis carried out based on MK-CPFE model, the shape of the yield surface for the steel sheet is determined based on the initial texture evolution, and the mechanical properties of constituent phases. Consequently, the individual phase property has one of the most important impacts on the FLC prediction. It can be noticed that ferrite may have an effect on the predicted limit strain and subsequently on FLC more than other phases. This agrees well with DIC measurements when localization in many cases tend to concentrate where ferrite phases are [59].

5.3. FLC validation with the T-shape component CPFE simulation The T-shape stamping was used to evaluate the formability of the QP980 steel sheet under complex forming conditions. The maximum punch stroke without tearing or splitting the sheet was taken as a relative formability index for different test setups. 39

The CPFE simulation of T-shape stamping process was conducted with two different 1.0 mm thick QP980 steel sheets. Failure strains were calculated based on the FLC predicted by the multiphase CPFE model discussed in Section 5.2.

Fig. 15 shows the FE model of the die, punch, blank and blank holder used in the T-shape simulation. Analytical rigid body surfaces were utilized for the die, blank holder and the punch. Blanks were meshed with 0.333 mm × 1 mm elements size (three layers through the thickness) and C3D8R element type from the ABAQUS/Explicit element library [69]. It is well known that computational times increase almost quadratically by increasing element number [3]. Also, reducing the size of the blank element will require additional mesh refinement for the T-shape part, and subsequently increase the computational time required by the microstructure-based CPFE model. Hence, it is important to mention here that multiphase CPFE model was less sensitive to changes made in the element size compared with phenomenological models under large deformation applications [59]. Therefore, additional mesh refinement below 1.0 mm (surface element size) and 0.333 mm (thickness element size) was not considered in this study.

Fig. 15: Schematic diagram for Finite element model of a T-shape component stamping simulation. 40

The Coulomb friction model was used to describe the contact interaction between the rigid body tooling and the deformable blank. A friction coefficient of 0.12 was assumed in the CPFE simulation, as it showed the best fit to the experimental punch force-stroke relationship. Furthermore, since a strain-rate independent material model was assumed in the finite element simulations, and to enhance the calculation speed, mass-scaling was used by setting the minimum step increment time to 10-7 seconds [69]. Stamping simulation of a T-shape was also carried out using the CPFE model with 140 grain orientations per integration point. In addition, the random volume fraction distribution and orientations of the phases were assumed for the sheet metal.

Fig. 16(a) and (b) illustrate the contour plot of the equivalent plastic strain and the corresponding experimental results, respectively, when the punch force reaches the peak value in the T-shape stamping of sample-1, as shown in Fig. 16(c).

(a)

(b)

41

(c)

Fig. 16: CPFE simulation and experimental results of the T-shape stamping sample-1. (a) Equivalent plastic strain distribution based on CPFE model; (b) Experimental final shape results; (c) Comparison of punch force versus punch stroke relationship during the stamping process.

Visual inspection of experimentally stamped T-shape, Fig. 16(b), showed that the part did not fail. It can be seen from simulation results, Fig. 16(a), that plastic strains are highest in the corner areas of the T-shape part where there is severe bending and stretching deformations. However, failure of the T-shape part could not be ascertained by visual inspection of the simulation results alone. Therefore, major and minor strains at the final punch depth, Fig. 16 (c), were calculated from the strain components and plotted on the forming limit diagram (FLD), as shown in Fig. 17.

42

Fig. 17: The minor and major true strain distributions and FLC predicted by CPFE model of T-shape sample-1 at the end of stamping process.

Strains with critical values from multiple regions (elements) with different colors (upper-right corner of Fig. 17) for the simulated T-shape were projected onto the FLD as shown in Fig. 17. According to the simulation results, and compared with the FLC predicted with CPFE model, some of the major and minor strains plotted on the FLD indicate that the stamped T-shape might be experiencing necking. From the experimental perspective, cracks and wrinkles are the type of failures that can be predicted from simulation results using fracture forming limit curve (FFLC) instead of FLC [73]. Hence, the onset of necking cannot be identified just from visual inspection, without experimentally measured forming strains. In addition, the critical strains that crossed the FLC in Fig. 17 may have been due to the slightly larger punch force predicted at the end of the simulation result, as shown in Fig. 16(c). However, overall, the predicted punch force-stroke curve based on the CPFE model and 0.12-friction coefficient is in good agreement with the experimental curve, Fig. 16(c).

The simulation results with the contour of the equivalent plastic strain and the experimental final shape of the T-shape (sample-2) with holes, are shown in Fig. 18(a) and (b), respectively. 43

Here, the simulation results from Fig. 18(a) at ~17.5 mm punch stroke cannot be used for formability assessment because the experimental punch force-stroke curve showed earlier fracture at approximately 14.3 mm punch depth, Fig. 18(c). Therefore, the strains were collected for three punch depths prior to the maximum load occurring at the 14.3 mm punch depth.

(a)

(b)

(c) 44

Fig. 18: CPFE simulation and experimental results of the T-shape stamping sample-2. (a) Equivalent plastic strain distribution based on CPFE model; (b) Experimental final shape results; (c) Comparison of punch force versus punch stroke relationship during the stamping process.

For the safe T-shape component stamping at 12.5 mm punch depth, Fig. 18(c), it was noticed that true strains everywhere in the sheet were less than the critical limit strains as defined by FLC in Fig. 19(a). Also, it was observed that the maximum plastic deformation generated around the holes with no contact surfaces, gradually extended to adjacent regions around the holes as the stamping process progressed to 13.5 mm punch depth, as shown in Fig. 19(b), when the sheet started to experience the onset of necking around the holes. At approximately 14 mm punch depth, the CPFE punch force-stroke curve overestimates the experimental curve. The calculated strains plotted on the FLD in Fig. 19(c) at 14.0 mm punch depth, indicate that the sheet metal is close to fracture since many of the strain points are above the FLC with additional critical strains also occurring at locations away from the holes.

(a) 45

(b)

(c) 46

Fig. 19: The minor and major true strain distributions and FLC predicted by CPFE model of T-shape sample-2 at punch depth (a) 12.5 mm; (b) 13.5 mm and (c) 14.0 mm.

As can be seen from these figures, the CPFE model was able to predict the safe strains, as well as necking strains and failure locations in the sheet at various conditions. However, it can be seen that fracture observed from the experimental test for sample-2, Fig. 18(c), occurred at an earlier punch stroke of 14.3 mm compared with the fracture from the punch force versus punch stroke curves predicted by the CPFE model. The CPFE model in this work was not intended to account for the material behavior beyond the strain localization. In other words, strain rate sensitivity and damage behavior with element deletion were not considered in this study. Also, the extended Voce type hardening rule shown in Eq. (7) converges to the linear hardening rule as the exponent part vanishes with the increasing accumulated shear strain. Therefore, the material model could not accurately predict the necking of the punch force versus punch stroke curves of sample-2.

6. Conclusions In this study, numerical procedure for predicting the forming-limit behavior of steel sheet metals is discussed within the framework of the MK technique using a multiphase computationally efficient rate independent CPFE model. According to all the observations on strain distribution in uniaxial tensile tests, formability tests and metallurgical analysis of the QP980 steel, it was found that the inconsistency of formability is attributed to the microstructural features of the sheet metal. Forming limit strains from the experiments associated with the onset of localized necking within a local area for specified deformation path cannot accurately represent the formability involved during a forming process. CPFE model, which accounts for the grain rotation and evolution of anisotropy, was used for the description of each phase’s mechanical behavior. Inhomogeneity of the sheet metal related to inhomogeneous distribution of phases, random orientations and artificial groove size within the sheet metal showed good prediction of FLC. The accurate prediction of strains at the onset of necking of the T-shape stamped part, offers a promising microstructure-sensitive model that will be highly desirable for the stamping simulation of the third-generation advance high strength steels.

47

Acknowledgements This material is based upon work supported by the Department of Energy under Cooperative Agreement Number DOE DE-EE000597, with United States Automotive Materials Partnership LLC (USAMP).

This report was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor any agency thereof, nor any of their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.

References [1]

D.K. Matlock, J.G. Speer, Third generation of AHSS: microstructure design concepts, 2009. doi:10.1007/978-1-84882-454-6_11.

[2]

M.Y. Demeri, Advanced high-strength Steels, 57 (2013) 1–31. doi:10.1007/978-3-64217665-4.

[3]

A.E. Tekkaya, State-of-the-art of simulation of sheet metal forming, J. Mater. Process. Technol. 103 (2000) 14–22. doi:10.1016/S0924-0136(00)00413-1.

[4]

C. Schwindt, F. Schlosser, M.A. Bertinetti, M. Stout, J.W. Signorelli, Experimental and Visco-Plastic Self-Consistent evaluation of forming limit diagrams for anisotropic sheet metals: An efficient and robust implementation of the M-K model, Int. J. Plast. 73 (2015) 62–99. doi:10.1016/j.ijplas.2015.01.005.

[5]

S.P. Keeler, Determination of Forming Limits in Automotive Stampings, SAE Tech. Pap. 14B (1965) 656–669. doi:10.4271/650535.

[6]

G.M. Goodwin, Application of strain analysis to sheet metal forming in the press shop, SAE Pap. 680093 (1968) 767–774.

[7]

M.J. Serenelli, M.A. Bertinetti, J.W. Signorelli, Study of limit strains for FCC and BCC sheet metal using polycrystal plasticity, Int. J. Solids Struct. 48 (2011) 1109–1119. doi:10.1016/j.ijsolstr.2010.12.013. 48

[8]

K. Janssens, F. Lambert, S. Vanrostenberghe, M. Vermeulen, Statistical evaluation of the uncertainty of experimentally characterised forming limits of sheet steel, J. Mater. Process. Technol. 112 (2001) 174–184. doi:10.1016/S0924-0136(00)00890-6.

[9]

H.W. Swift, Plastic instability under plane stress, J. Mech. Phys. Solids. 1 (1952) 1–18. doi:10.1016/0022-5096(52)90002-1.

[10] R. Hill, On discontinuous plastic states, with special reference to localized necking in thin sheets, J. Mech. Phys. Solids. 1 (1952) 19–30. doi:10.1016/0022-5096(52)900033. [11]

Z. Marciniak, K. Kuczyński, Limit strains in the processes of stretch-forming sheet metal, Int. J. Mech. Sci. 9 (1967) 609–620. doi:10.1016/0020-7403(67)90066-5.

[12] D. Banabic, A review on recent developments of Marciniak-Kuczynski model, Comput. Methods Mater. Sci. (2010) 1–24. [13] F. Barlat, K. Lian, Plastic behavior and stretchability of sheet metals. Part I: A yield function for orthotropic sheets under plane stress conditions, Int. J. Plast. 5 (1989) 51– 66. doi:10.1016/0749-6419(89)90019-3. [14] R. Hill, A Theory of the Yielding and Plastic Flow of Anisotropic Metals, Proc. R. Soc. London A Math. Phys. Eng. Sci. 193 (1948) 281–297. doi:10.1098/rspa.1948.0045. [15] R. Sowerby, J.L. Duncan, Failure in sheet metal in biaxial tension, Int. J. Mech. Sci. 13 (1971) 217–229. doi:10.1016/0020-7403(71)90004-X. [16] H.W. Graf Alejandro, The influence of strain-path changes on formint limit diagrams of Al 6111-T 4, Int. J. Mech. Sci. 36 (1994) 897–910. doi:10.1016/S09240136(02)00311-4. [17] A. Graf, W. Hosford, Effect of Changing Strain Paths on Forming Limit Diagrams of Al 2008-T4, Metall. Trans. a-Physical Metall. Mater. Sci. 24 (1993) 2503–2512. doi:10.1007/BF02646529. [18] W.F. Hosford, A Generalized Isotropic Yield Criterion, J. Appl. Mech. 39 (1972) 607. doi:10.1115/1.3422732. [19] F. Barlat, J.C. Brem, D.J. Lege, K. Chung, Advanced Methods in Materials Processing Defects, Stud. Appl. Mech. 45 (1997) 265–272. doi:10.1016/S0922-5382(97)80028-1. [20] J. Cao, H. Yao, A. Karafillis, M.C. Boyce, Prediction of localized thinning in sheet metal using a general anisotropic yield criterion, Int. J. Plast. 16 (2000) 1105–1129. doi:10.1016/S0749-6419(99)00091-1. [21] A.P. Karafillis, M.C. Boyce, A general anisotropic yield criterion using bounds and a transformation weighting tensor, J. Mech. Phys. Solids. 41 (1993) 1859–1886. doi:10.1016/0022-5096(93)90073-O. [22] A.F. Ávila, E.L.S. Vieira, Proposing a better forming limit diagram prediction: A 49

comparative study, J. Mater. Process. doi:10.1016/S0924-0136(03)00162-6.

Technol.

141

(2003)

101–108.

[23] T.B. Stoughton, X. Zhu, Review of theoretical models of the strain-based FLD and their relevance to the stress-based FLD, Int. J. Plast. 20 (2004) 1463–1486. doi:10.1016/j.ijplas.2003.11.004. [24] S. Soare, D. Banabic, A discussion upon the sensitivity of the MK model to input data, Int. J. Mater. Form. 2 (2009) 503–506. doi:10.1007/s12289-009-0521-x. [25] P. Eyckens, A. Van Bael, P. Van Houtte, Marciniak-Kuczynski type modelling of the effect of Through-Thickness Shear on the forming limits of sheet metal, Int. J. Plast. 25 (2009) 2249–2268. doi:10.1016/j.ijplas.2009.02.002. [26] S. Ahmadi, A.R. Eivani, A. Akbarzadeh, An experimental and theoretical study on the prediction of forming limit diagrams using new BBC yield criteria and M-K analysis, Comput. Mater. Sci. 44 (2009) 1272–1280. doi:10.1016/j.commatsci.2008.08.013. [27] A.A. Zadpoor, J. Sinke, R. Benedictus, Formability prediction of high strength aluminum sheets, Int. J. Plast. 25 (2009) 2269–2297. doi:10.1016/j.ijplas.2009.02.005. [28] P. Eyckens, A. Van Bael, P. Van Houtte, An extended Marciniak-Kuczynski model for anisotropic sheet subjected to monotonic strain paths with through-thickness shear, Int. J. Plast. 27 (2011) 1577–1597. doi:10.1016/j.ijplas.2011.03.008. [29] S. Panich, F. Barlat, V. Uthaisangsuk, S. Suranuntchai, S. Jirathearanat, Experimental and theoretical formability analysis using strain and stress based forming limit diagram for advanced high strength steels, Mater. Des. 51 (2013) 756–766. doi:10.1016/j.matdes.2013.04.080. [30] F. Zhang, J. Chen, J. Chen, Effect of through-thickness normal stress on forming limits under Yld2003 yield criterion and M-K model, Int. J. Mech. Sci. 89 (2014) 92–100. doi:10.1016/j.ijmecsci.2014.08.024. [31] P. Eyckens, H. Mulder, J. Gawad, H. Vegter, D. Roose, T. van den Boogaard, A. Van Bael, P. Van Houtte, The prediction of differential hardening behaviour of steels by multi-scale crystal plasticity modelling, Int. J. Plast. 73 (2015) 1–23. doi:10.1016/j.ijplas.2014.12.004. [32] R. Wagoner, K. Chan, S. Keeler, Forming Limit Diagrams: Concepts, Methods and Applications, 1989. [33] K. Narasimhan, R.H. Wagoner, Finite element modeling simulation of in-plane forming limit diagrams of sheets containing finite defects, Metall. Trans. A. 22 (1991) 2655–2665. doi:10.1007/BF02851359. [34] S.H. Evangelista, J. Lirani, H.A. Al-Qureshi, Implementing a modified MarciniakKuczynski model using the finite element method for the simulation of sheet metal deep drawing, J. Mater. Process. Technol. 130–131 (2002) 135–144. 50

doi:10.1016/S0924-0136(02)00729-X. [35] A.H. Van Den Boogaard, J. Hu, Prediction of sheet necking with shell finite element models, (n.d.). [36] C. Zhang, L. Leotoing, G. Zhao, D. Guines, E. Ragneau, A methodology for evaluating sheet formability combining the tensile test with the M-K model, Mater. Sci. Eng. A. 528 (2010) 480–485. doi:10.1016/j.msea.2010.09.001. [37] A. Srivastava, A.F. Bower, L.G. Hector, J.E. Carsley, L. Zhang, F. Abu-Farha, A multiscale approach to modeling formability of dual-phase steels, Model. Simul. Mater. Sci. Eng. 24 (2016) 25011. doi:10.1088/0965-0393/24/2/025011. [38] E. Cyr, M. Mohammadi, A. Brahme, R.K. Mishra, K. Inal, Modeling the formability of aluminum alloys at elevated temperatures using a new thermo-elasto-viscoplastic crystal plasticity framework, Int. J. Mech. Sci. 128–129 (2017) 312–325. doi:10.1016/j.ijmecsci.2017.05.005. [39] R.J. Asaro, A. Needleman, Overview no. 42 Texture development and strain hardening in rate dependent polycrystals, Acta Metall. 33 (1985) 923–953. doi:10.1016/00016160(85)90188-9. [40] Y. Zhou, K.W. Neale, Predictions of forming limit diagrams using a rate-sensitive crystal plasticity model, Int. J. Mech. Sci. 37 (1995) 1–20. doi:10.1016/00207403(94)00052-L. [41] P.D. Wu, S.R. MacEwen, D.J. Lloyd, K.W. Neale, A mesoscopic approach for predicting sheet metal formability, Model. Simul. Mater. Sci. Eng. 12 (2004) 511–527. doi:10.1088/0965-0393/12/3/011. [42] P.D. Wu, A. Graf, S.R. MacEwen, D.J. Lloyd, M. Jain, K.W. Neale, On forming limit stress diagram analysis, Int. J. Solids Struct. 42 (2005) 2225–2241. doi:10.1016/j.ijsolstr.2004.09.010. [43] P.D. Wu, K.W. Neale, E. Giessen, M. Jain, S.R. MacEwen, a. Makinde, Crystal plasticity forming limit diagram analysis of rolled aluminum sheets, Metall. Mater. Trans. A. 29 (1998) 527–535. doi:10.1007/s11661-998-0134-x. [44] P.D. Wu, K.W. Neale, E. Van Der Giessen, On Crystal Plasticity FLD Analysis, Proc. R. Soc. London A. 453 (1997) 1831–1848. doi:10.1098/rspa.1997.0099. [45] K. Inal, K.W. Neale, a. Aboutajeddine, Forming limit comparisons for FCC and BCC sheets, Int. J. Plast. 21 (2005) 1255–1266. doi:10.1016/j.ijplas.2004.08.001. [46] K. Yoshida, T. Ishizaka, M. Kuroda, S. Ikawa, The effects of texture on formability of aluminum alloy sheets, Acta Mater. 55 (2007) 4499–4506. doi:10.1016/j.actamat.2007.04.014. [47] J.W. Signorelli, M.A. Bertinetti, On the role of constitutive model in the forming limit 51

of FCC sheet metal with cube orientations, Int. J. Mech. Sci. 51 (2009) 473–480. doi:10.1016/j.ijmecsci.2009.04.002. [48] C. John Neil, S.R. Agnew, Crystal plasticity-based forming limit prediction for noncubic metals: Application to Mg alloy AZ31B, Int. J. Plast. 25 (2009) 379–398. doi:10.1016/j.ijplas.2008.05.003. [49] M. Yang, X. Dong, R. Zhou, J. Cao, Crystal plasticity-based forming limit prediction for FCC materials under non-proportional strain-path, Mater. Sci. Eng. A. 527 (2010) 6607–6613. doi:10.1016/j.msea.2010.06.063. [50] H. Wang, P.D. Wu, K.P. Boyle, K.W. Neale, On crystal plasticity formability analysis for magnesium alloy sheets, Int. J. Solids Struct. 48 (2011) 1000–1010. doi:10.1016/j.ijsolstr.2010.12.004. [51] K. Yoshida, M. Kuroda, Comparison of bifurcation and imperfection analyses of localized necking in rate-independent polycrystalline sheets, Int. J. Solids Struct. 49 (2012) 2073–2084. doi:10.1016/j.ijsolstr.2012.04.010. [52] R. Chiba, H. Takeuchi, M. Kuroda, T. Hakoyama, T. Kuwabara, Theoretical and experimental study of forming-limit strain of half-hard AA1100 aluminium alloy sheet, Comput. Mater. Sci. 77 (2013) 61–71. doi:10.1016/j.commatsci.2013.04.025. [53] J.H. Kim, M.G. Lee, D. Kim, F. Barlat, Numerical procedures for predicting localization in sheet metals using crystal plasticity, Comput. Mater. Sci. 72 (2013) 107–115. doi:10.1016/j.commatsci.2013.02.008. [54] M. Mohammadi, A.P. Brahme, R.K. Mishra, K. Inal, Effects of post-necking hardening behavior and equivalent stress-strain curves on the accuracy of M-K based forming limit diagrams, Comput. Mater. Sci. 85 (2014) 316–323. doi:10.1016/j.commatsci.2014.01.017. [55] J. Lévesque, M. Mohammadi, R.K. Mishra, K. Inal, An extended Taylor model to simulate localized deformation phenomena in magnesium alloys, Int. J. Plast. 78 (2015). doi:10.1016/j.ijplas.2015.10.012. [56] C.D. Schwindt, M.A. Bertinetti, L. Iurman, C.A. Rossit, J.W. Signorelli, Numerical study of the effect of martensite plasticity on the forming limits of a dual-phase steel sheet, Int. J. Mater. Form. (2015) 499–517. doi:10.1007/s12289-015-1236-9. [57] L. Wang, J.G. Speer, Quenching and Partitioning Steel Heat Treatment, Metallogr. Microstruct. Anal. 2 (2013) 268–281. doi:10.1007/s13632-013-0082-8. [58] L. Zhang, J. Lin, J. Min, Y. Ye, L. Kang, Formability Evaluation of Sheet Metals Based on Global Strain Distribution, J. Mater. Eng. Perform. 25 (2016) 1–11. doi:10.1007/s11665-016-2054-z. [59] B. Mohammed, T. Park, F. Pourboghrat, J. Hu, R. Esmaeilpour, F. Abu-Farha, Multiscale Crystal Plasticity Modeling of Multiphase Advanced High Strength Steel, 52

Int. J. Solids Struct. (2017). doi:10.1016/j.ijsolstr.2017.05.007. [60] A.R. Zamiri, F. Pourboghrat, A novel yield function for single crystals based on combined constraints optimization, Int. J. Plast. 26 (2010) 731–746. doi:10.1016/j.ijplas.2009.10.004. [61] C. Tome, G.R. Canova, U.F. Kocks, N. Christodoulou, J.J. Jonas, The relation between macroscopic and microscopic strain hardening in F.C.C. polycrystals, Acta Metall. 32 (1984) 1637–1653. doi:10.1016/0001-6160(84)90222-0. [62] A. Zamiri, F. Pourboghrat, F. Barlat, An effective computational algorithm for rateindependent crystal plasticity based on a single crystal yield surface with an application to tube hydroforming, Int. J. Plast. 23 (2007) 1126–1147. doi:10.1016/j.ijplas.2006.10.012. [63] H.J. Bunge, Texture analysis in materials science, Butterworth., 1982. [64] ASTM Int., Standard Test Methods for Tension Testing of Metallic Materials 1, Astm. (2009) 1–27. doi:10.1520/E0008. [65] International Standard ISO 12004-2, Metallic Materials-sheet and Strip Determination of Forming Limit Curves. Part 2: Determination of Forming Limit Curves in the Laboratory. International Organization for Standardization, Geneva, Switzerland., (2008). [66] X. Hu, K.S. Choi, X. Sun, Y. Ren, Y. Wang, Determining Individual Phase Flow Properties in a Quench and Partitioning Steel with In Situ High-Energy X-Ray Diffraction and Multiphase Elasto-Plastic Self-Consistent Method, Metall. Mater. Trans. A Phys. Metall. Mater. Sci. (2016) 1–17. doi:10.1007/s11661-016-3373-2. [67] X.H. Hu, X. Sun, L.G. Hector, Y. Ren, Individual phase constitutive properties of a TRIP-assisted QP980 steel from a combined synchrotron X-ray diffraction and crystal plasticity approach, Acta Mater. 132 (2017) 230–244. doi:10.1016/j.actamat.2017.04.028. [68] Y. Guan, F. Pourboghrat, F. Barlat, Finite element modeling of tube hydroforming of polycrystalline aluminum alloy extrusions, Int. J. Plast. 22 (2006) 2366–2393. doi:10.1016/j.ijplas.2006.04.003. [69] ABAQUS User’s Manual, version 6.14, Hibbit, Karlsson & Sorenson, Providence, RI., (2000). [70] S. Sodjit, V. Uthaisangsuk, Microstructure based prediction of strain hardening behavior of dual phase steels, Mater. Des. 41 (2012) 370–379. doi:10.1016/j.matdes.2012.05.010. [71] J. Lian, F. Barlat, B. Baudelet, Plastic behaviour and stretchability of sheet metals. Part II: Effect of yield surface shape on sheet forming limit, Int. J. Plast. 5 (1989) 131–147. doi:10.1016/0749-6419(89)90026-0. 53

[72] K.W. Hutchinson, J. W., Neale, Sheet Necking II: time independent behaviour, in: Koistinen K. P., Wang N. -M. (Eds.), Mech. Sheet Met. Forming, Plenum, New York. (1978) 127–153. [73] K. Chung, C. Lee, H. Kim, Forming limit criterion for ductile anisotropic sheets as a material property and its deformation path insensitivity, Part II: Boundary value problems, Int. J. Plast. 58 (2014) 35–65. doi:10.1016/j.ijplas.2014.03.014.

54